 
data_1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H36 La2 Mo6 O44 V2' 
_chemical_formula_weight          1695.63 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'La'  'La'  -0.2871   2.4523 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    10.0427(4) 
_cell_length_b                    10.1151(4) 
_cell_length_c                    19.7105(8) 
_cell_angle_alpha                 77.558(2) 
_cell_angle_beta                  82.638(2) 
_cell_angle_gamma                 78.650(2) 
_cell_volume                      1909.29(13) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     293(2) 
_cell_measurement_reflns_used     10896  
_cell_measurement_theta_min       2.09 
_cell_measurement_theta_max       25.00 
 
_exptl_crystal_description        'block'
_exptl_crystal_colour             'yellow' 
_exptl_crystal_size_max           0.29 
_exptl_crystal_size_mid           0.18 
_exptl_crystal_size_min           0.17 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.949 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1600 
_exptl_absorpt_coefficient_mu     4.677 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.379
_exptl_absorpt_correction_T_max   0.452  
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995' 
  
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       293(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ'
_diffrn_detector_area_resol_mean  0.01 
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0 
_diffrn_standards_interval_time   0 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             10896 
_diffrn_reflns_av_R_equivalents   0.0195 
_diffrn_reflns_av_sigmaI/netI     0.0325 
_diffrn_reflns_limit_h_min        -11 
_diffrn_reflns_limit_h_max        11 
_diffrn_reflns_limit_k_min        -12 
_diffrn_reflns_limit_k_max        10 
_diffrn_reflns_limit_l_min        -23 
_diffrn_reflns_limit_l_max        23 
_diffrn_reflns_theta_min          2.09 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              6693 
_reflns_number_gt                 5584 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL'
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0283P)²+7.5352P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.'
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          6693 
_refine_ls_number_parameters      487 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0362 
_refine_ls_R_factor_gt            0.0287 
_refine_ls_wR_factor_ref          0.0745 
_refine_ls_wR_factor_gt           0.0687 
_refine_ls_goodness_of_fit_ref    1.044 
_refine_ls_restrained_S_all       1.044 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
La1 La 0.70530(3) 0.63395(3) 0.128295(17) 0.01758(9) Uani 1 1 d . . . 
La2 La 1.28977(3) -0.09240(3) 0.370660(17) 0.01790(9) Uani 1 1 d . . . 
Mo1 Mo 1.01018(5) 0.54500(5) 0.24775(2) 0.01601(11) Uani 1 1 d . . . 
Mo2 Mo 0.72880(5) 0.47780(5) 0.33292(3) 0.01863(12) Uani 1 1 d . . . 
Mo3 Mo 0.72349(5) 0.25400(5) 0.24019(2) 0.01567(11) Uani 1 1 d . . . 
Mo4 Mo 0.98264(5) -0.00418(5) 0.25142(2) 0.01602(11) Uani 1 1 d . . . 
Mo5 Mo 1.26091(5) 0.06411(5) 0.16516(2) 0.01917(12) Uani 1 1 d . . . 
Mo6 Mo 1.26771(5) 0.28716(5) 0.25771(2) 0.01599(11) Uani 1 1 d . . . 
V1 V 1.00365(9) 0.31835(9) 0.15932(4) 0.01187(19) Uani 1 1 d . . . 
V2 V 0.98654(9) 0.22367(9) 0.33928(4) 0.01178(19) Uani 1 1 d . . . 
O1 O 0.8871(4) 0.3756(4) 0.25294(19) 0.0156(8) Uani 1 1 d . . . 
O2 O 0.6372(4) 0.5185(4) 0.4059(2) 0.0318(10) Uani 1 1 d . . . 
O3 O 1.3355(4) 0.1489(4) 0.3192(2) 0.0199(8) Uani 1 1 d . . . 
O4 O 0.8826(4) 0.1834(3) 0.18110(18) 0.0145(8) Uani 1 1 d . . . 
O5 O 1.1084(4) 0.3568(4) 0.31790(18) 0.0149(8) Uani 1 1 d . . . 
O6 O 0.9125(4) 0.4398(4) 0.1072(2) 0.0197(8) Uani 1 1 d . . . 
O7 O 1.0769(4) 0.1017(4) 0.39102(19) 0.0192(8) Uani 1 1 d . . . 
O8 O 1.3380(4) 0.2181(4) 0.1750(2) 0.0208(9) Uani 1 1 d . . . 
O9 O 1.0808(4) -0.1080(4) 0.31508(19) 0.0201(8) Uani 1 1 d . . . 
O10 O 0.8693(4) 0.1161(4) 0.31162(19) 0.0162(8) Uani 1 1 d . . . 
O11 O 0.8664(4) 0.3065(4) 0.39196(19) 0.0190(8) Uani 1 1 d . . . 
O12 O 1.3646(4) 0.4101(4) 0.2528(2) 0.0271(10) Uani 1 1 d . . . 
O13 O 1.1039(4) -0.0213(4) 0.17031(19) 0.0205(9) Uani 1 1 d . . . 
O14 O 0.6520(4) 0.5928(4) 0.2634(2) 0.0250(9) Uani 1 1 d . . . 
O15 O 0.8861(4) 0.5634(4) 0.32840(19) 0.0203(9) Uani 1 1 d . . . 
O16 O 1.1050(4) 0.1663(4) 0.24496(19) 0.0160(8) Uani 1 1 d . . . 
O17 O 0.9142(4) 0.6503(4) 0.1832(2) 0.0196(8) Uani 1 1 d . . . 
O18 O 1.1234(4) 0.2342(4) 0.10718(19) 0.0182(8) Uani 1 1 d . . . 
O19 O 1.1218(4) 0.4257(4) 0.18671(18) 0.0155(8) Uani 1 1 d . . . 
O20 O 1.3339(4) -0.0497(4) 0.2340(2) 0.0250(9) Uani 1 1 d . . . 
O21 O 0.6524(4) 0.3237(4) 0.32215(19) 0.0200(8) Uani 1 1 d . . . 
O22 O 0.6578(4) 0.3906(4) 0.1772(2) 0.0211(9) Uani 1 1 d . . . 
O23 O 1.1303(4) 0.6347(4) 0.2585(2) 0.0279(10) Uani 1 1 d . . . 
O24 O 0.8627(4) -0.0957(4) 0.2433(2) 0.0264(10) Uani 1 1 d . . . 
O25 O 0.6282(4) 0.1316(4) 0.2438(2) 0.0257(9) Uani 1 1 d . . . 
O26 O 1.3516(4) 0.0232(4) 0.0909(2) 0.0318(10) Uani 1 1 d . . . 
O1W O 0.8628(5) 0.7511(5) 0.0350(2) 0.0328(10) Uani 1 1 d . . . 
O2W O 0.4484(5) 0.6352(5) 0.1569(3) 0.0400(12) Uani 1 1 d . . . 
O3W O 0.6676(5) 0.8644(4) 0.1663(2) 0.0385(12) Uani 1 1 d . . . 
O4W O 0.5611(5) 0.8257(4) 0.0455(2) 0.0314(10) Uani 1 1 d . . . 
O5W O 0.6557(5) 0.5500(5) 0.0242(2) 0.0397(12) Uani 1 1 d . . . 
O6W O 1.4291(5) -0.2787(4) 0.4542(2) 0.0347(11) Uani 1 1 d . . . 
O7W O 1.3589(5) 0.0128(4) 0.4612(2) 0.0328(11) Uani 1 1 d . . . 
O8W O 1.3437(5) -0.3230(4) 0.3270(3) 0.0414(13) Uani 1 1 d . . . 
O9W O 1.1323(5) -0.2186(6) 0.4618(3) 0.0539(15) Uani 1 1 d . . . 
O10W O 1.5422(4) -0.1083(5) 0.3292(2) 0.0382(11) Uani 1 1 d . . . 
OW1 O 0.5262(5) 0.3047(5) 0.0704(2) 0.0385(11) Uani 1 1 d . . . 
OW2 O 0.4566(5) 0.2570(5) 0.4312(2) 0.0381(11) Uani 1 1 d . . . 
OW3 O 0.2458(5) 0.6009(5) 0.0777(3) 0.0460(13) Uani 1 1 d . . . 
OW4 O 0.7281(5) 0.9410(5) 0.4096(2) 0.0452(13) Uani 1 1 d . . . 
OW5 O 0.9002(5) 0.6904(6) 0.4406(3) 0.0475(13) Uani 1 1 d . . . 
OW6 O 0.0840(5) 0.8611(6) 0.0541(3) 0.0476(13) Uani 1 1 d . . . 
OW7 O 0.2056(6) 0.4416(6) 0.4290(3) 0.0547(14) Uani 1 1 d . . . 
OW8 O 0.7590(6) 0.0942(5) 0.0750(3) 0.0493(13) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
La1 O1W 2.518(4) . ? 
La1 O5W 2.521(4) . ? 
La1 O17 2.530(4) . ? 
La1 O3W 2.544(4) . ? 
La1 O22 2.557(4) . ? 
La1 O2W 2.568(4) . ? 
La1 O4W 2.580(4) . ? 
La1 O14 2.607(4) . ? 
La1 O6 2.623(4) . ? 
La2 O7W 2.496(4) . ? 
La2 O6W 2.537(4) . ? 
La2 O9 2.535(4) . ? 
La2 O9W 2.537(5) . ? 
La2 O3 2.541(4) . ? 
La2 O10W 2.546(4) . ? 
La2 O8W 2.593(4) . ? 
La2 O20 2.628(4) . ? 
La2 O7 2.656(4) . ? 
Mo1 O23 1.703(4) . ? 
Mo1 O17 1.734(4) . ? 
Mo1 O15 1.909(4) . ? 
Mo1 O19 1.977(4) . ? 
Mo1 O5 2.233(4) . ? 
Mo1 O1 2.280(4) . ? 
Mo1 Mo2 3.2115(7) . ? 
Mo2 O2 1.689(4) . ? 
Mo2 O14 1.748(4) . ? 
Mo2 O15 1.929(4) . ? 
Mo2 O21 1.928(4) . ? 
Mo2 O11 2.206(4) . ? 
Mo2 O1 2.343(4) . ? 
Mo2 Mo3 3.2130(7) . ? 
Mo3 O25 1.692(4) . ? 
Mo3 O22 1.731(4) . ? 
Mo3 O21 1.901(4) . ? 
Mo3 O4 1.963(4) . ? 
Mo3 O10 2.225(4) . ? 
Mo3 O1 2.305(4) . ? 
Mo3 V1 3.1630(10) . ? 
Mo4 O24 1.699(4) . ? 
Mo4 O9 1.729(4) . ? 
Mo4 O13 1.899(4) . ? 
Mo4 O10 1.979(4) . ? 
Mo4 O4 2.237(4) . ? 
Mo4 O16 2.281(4) . ? 
Mo4 Mo5 3.1959(7) . ? 
Mo5 O26 1.707(4) . ? 
Mo5 O20 1.719(4) . ? 
Mo5 O13 1.923(4) . ? 
Mo5 O8 1.925(4) . ? 
Mo5 O18 2.190(4) . ? 
Mo5 O16 2.330(4) . ? 
Mo5 Mo6 3.2076(7) . ? 
Mo6 O12 1.703(4) . ? 
Mo6 O3 1.730(4) . ? 
Mo6 O8 1.910(4) . ? 
Mo6 O5 1.973(4) . ? 
Mo6 O19 2.223(4) . ? 
Mo6 O16 2.291(4) . ? 
V1 O6 1.630(4) . ? 
V1 O18 1.698(4) . ? 
V1 O19 1.950(4) . ? 
V1 O4 1.947(4) . ? 
V1 O1 2.180(4) . ? 
V1 O16 2.226(4) . ? 
V2 O7 1.625(4) . ? 
V2 O11 1.700(4) . ? 
V2 O5 1.939(4) . ? 
V2 O10 1.948(4) . ? 
V2 O16 2.199(4) . ? 
V2 O1 2.227(4) . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1W La1 O5W 79.92(15) . . ? 
O1W La1 O17 71.69(13) . . ? 
O5W La1 O17 137.03(14) . . ? 
O1W La1 O3W 81.62(15) . . ? 
O5W La1 O3W 135.93(15) . . ? 
O17 La1 O3W 71.21(14) . . ? 
O1W La1 O22 138.11(13) . . ? 
O5W La1 O22 75.21(14) . . ? 
O17 La1 O22 105.63(12) . . ? 
O3W La1 O22 138.57(14) . . ? 
O1W La1 O2W 138.46(15) . . ? 
O5W La1 O2W 80.38(16) . . ? 
O17 La1 O2W 141.22(14) . . ? 
O3W La1 O2W 87.76(16) . . ? 
O22 La1 O2W 69.10(14) . . ? 
O1W La1 O4W 71.15(15) . . ? 
O5W La1 O4W 68.36(14) . . ? 
O17 La1 O4W 127.52(13) . . ? 
O3W La1 O4W 67.86(14) . . ? 
O22 La1 O4W 126.77(14) . . ? 
O2W La1 O4W 67.65(15) . . ? 
O1W La1 O14 139.34(13) . . ? 
O5W La1 O14 140.14(15) . . ? 
O17 La1 O14 71.03(12) . . ? 
O3W La1 O14 71.53(14) . . ? 
O22 La1 O14 68.72(12) . . ? 
O2W La1 O14 71.50(14) . . ? 
O4W La1 O14 122.22(13) . . ? 
O1W La1 O6 75.09(13) . . ? 
O5W La1 O6 74.63(13) . . ? 
O17 La1 O6 67.40(12) . . ? 
O3W La1 O6 137.04(14) . . ? 
O22 La1 O6 66.15(12) . . ? 
O2W La1 O6 132.81(14) . . ? 
O4W La1 O6 133.18(12) . . ? 
O14 La1 O6 104.55(12) . . ? 
O7W La2 O6W 71.00(14) . . ? 
O7W La2 O9 141.23(14) . . ? 
O6W La2 O9 128.01(14) . . ? 
O7W La2 O9W 90.36(17) . . ? 
O6W La2 O9W 70.10(16) . . ? 
O9 La2 O9W 70.85(14) . . ? 
O7W La2 O3 69.15(13) . . ? 
O6W La2 O3 127.61(14) . . ? 
O9 La2 O3 104.31(12) . . ? 
O9W La2 O3 140.95(16) . . ? 
O7W La2 O10W 81.89(16) . . ? 
O6W La2 O10W 70.26(15) . . ? 
O9 La2 O10W 133.97(14) . . ? 
O9W La2 O10W 139.99(16) . . ? 
O3 La2 O10W 71.69(13) . . ? 
O7W La2 O8W 139.14(14) . . ? 
O6W La2 O8W 68.83(14) . . ? 
O9 La2 O8W 73.61(13) . . ? 
O9W La2 O8W 83.02(19) . . ? 
O3 La2 O8W 134.14(15) . . ? 
O10W La2 O8W 77.98(16) . . ? 
O7W La2 O20 133.05(14) . . ? 
O6W La2 O20 124.93(13) . . ? 
O9 La2 O20 68.77(12) . . ? 
O9W La2 O20 135.81(15) . . ? 
O3 La2 O20 67.86(12) . . ? 
O10W La2 O20 67.56(14) . . ? 
O8W La2 O20 69.12(14) . . ? 
O7W La2 O7 76.60(13) . . ? 
O6W La2 O7 132.38(13) . . ? 
O9 La2 O7 66.28(11) . . ? 
O9W La2 O7 76.28(15) . . ? 
O3 La2 O7 66.98(12) . . ? 
O10W La2 O7 137.93(14) . . ? 
O8W La2 O7 138.97(13) . . ? 
O20 La2 O7 102.69(12) . . ? 
O23 Mo1 O17 105.83(19) . . ? 
O23 Mo1 O15 101.44(18) . . ? 
O17 Mo1 O15 100.41(17) . . ? 
O23 Mo1 O19 99.07(17) . . ? 
O17 Mo1 O19 95.90(16) . . ? 
O15 Mo1 O19 149.10(15) . . ? 
O23 Mo1 O5 91.47(17) . . ? 
O17 Mo1 O5 161.05(15) . . ? 
O15 Mo1 O5 83.25(15) . . ? 
O19 Mo1 O5 73.33(14) . . ? 
O23 Mo1 O1 163.66(17) . . ? 
O17 Mo1 O1 90.24(15) . . ? 
O15 Mo1 O1 77.95(14) . . ? 
O19 Mo1 O1 75.91(14) . . ? 
O5 Mo1 O1 72.22(13) . . ? 
O23 Mo1 Mo2 134.81(14) . . ? 
O17 Mo1 Mo2 87.68(13) . . ? 
O15 Mo1 Mo2 33.40(11) . . ? 
O19 Mo1 Mo2 122.68(10) . . ? 
O5 Mo1 Mo2 85.41(9) . . ? 
O1 Mo1 Mo2 46.82(9) . . ? 
O2 Mo2 O14 105.7(2) . . ? 
O2 Mo2 O15 102.25(19) . . ? 
O14 Mo2 O15 96.90(18) . . ? 
O2 Mo2 O21 101.32(19) . . ? 
O14 Mo2 O21 95.23(18) . . ? 
O15 Mo2 O21 149.41(15) . . ? 
O2 Mo2 O11 93.10(18) . . ? 
O14 Mo2 O11 161.19(16) . . ? 
O15 Mo2 O11 79.90(15) . . ? 
O21 Mo2 O11 79.61(15) . . ? 
O2 Mo2 O1 164.88(17) . . ? 
O14 Mo2 O1 89.44(16) . . ? 
O15 Mo2 O1 75.99(14) . . ? 
O21 Mo2 O1 76.15(14) . . ? 
O11 Mo2 O1 71.78(13) . . ? 
O2 Mo2 Mo1 135.20(16) . . ? 
O14 Mo2 Mo1 84.85(14) . . ? 
O15 Mo2 Mo1 33.00(11) . . ? 
O21 Mo2 Mo1 121.34(11) . . ? 
O11 Mo2 Mo1 82.57(10) . . ? 
O1 Mo2 Mo1 45.20(9) . . ? 
O2 Mo2 Mo3 133.93(16) . . ? 
O14 Mo2 Mo3 83.42(13) . . ? 
O15 Mo2 Mo3 121.75(11) . . ? 
O21 Mo2 Mo3 32.70(11) . . ? 
O11 Mo2 Mo3 82.65(9) . . ? 
O1 Mo2 Mo3 45.77(9) . . ? 
Mo1 Mo2 Mo3 89.926(17) . . ? 
O25 Mo3 O22 105.21(19) . . ? 
O25 Mo3 O21 101.81(18) . . ? 
O22 Mo3 O21 100.08(17) . . ? 
O25 Mo3 O4 99.10(17) . . ? 
O22 Mo3 O4 96.42(16) . . ? 
O21 Mo3 O4 148.82(15) . . ? 
O25 Mo3 O10 93.41(17) . . ? 
O22 Mo3 O10 160.09(16) . . ? 
O21 Mo3 O10 82.57(15) . . ? 
O4 Mo3 O10 73.30(14) . . ? 
O25 Mo3 O1 165.35(17) . . ? 
O22 Mo3 O1 89.21(16) . . ? 
O21 Mo3 O1 77.62(14) . . ? 
O4 Mo3 O1 76.33(13) . . ? 
O10 Mo3 O1 71.96(13) . . ? 
O25 Mo3 V1 134.66(14) . . ? 
O22 Mo3 V1 82.23(13) . . ? 
O21 Mo3 V1 121.19(12) . . ? 
O4 Mo3 V1 35.84(10) . . ? 
O10 Mo3 V1 79.63(9) . . ? 
O1 Mo3 V1 43.56(9) . . ? 
O25 Mo3 Mo2 134.92(14) . . ? 
O22 Mo3 Mo2 86.69(13) . . ? 
O21 Mo3 Mo2 33.23(11) . . ? 
O4 Mo3 Mo2 123.04(10) . . ? 
O10 Mo3 Mo2 85.01(9) . . ? 
O1 Mo3 Mo2 46.77(9) . . ? 
V1 Mo3 Mo2 89.45(2) . . ? 
O24 Mo4 O9 105.28(19) . . ? 
O24 Mo4 O13 102.29(18) . . ? 
O9 Mo4 O13 100.53(17) . . ? 
O24 Mo4 O10 97.92(17) . . ? 
O9 Mo4 O10 96.93(16) . . ? 
O13 Mo4 O10 148.63(16) . . ? 
O24 Mo4 O4 92.21(17) . . ? 
O9 Mo4 O4 160.94(15) . . ? 
O13 Mo4 O4 82.68(15) . . ? 
O10 Mo4 O4 72.74(14) . . ? 
O24 Mo4 O16 164.28(17) . . ? 
O9 Mo4 O16 90.03(16) . . ? 
O13 Mo4 O16 77.83(15) . . ? 
O10 Mo4 O16 76.30(14) . . ? 
O4 Mo4 O16 72.16(13) . . ? 
O24 Mo4 Mo5 135.72(14) . . ? 
O9 Mo4 Mo5 87.32(13) . . ? 
O13 Mo4 Mo5 33.50(11) . . ? 
O10 Mo4 Mo5 122.97(11) . . ? 
O4 Mo4 Mo5 85.28(9) . . ? 
O16 Mo4 Mo5 46.75(9) . . ? 
O26 Mo5 O20 106.71(19) . . ? 
O26 Mo5 O13 102.01(19) . . ? 
O20 Mo5 O13 95.80(18) . . ? 
O26 Mo5 O8 101.2(2) . . ? 
O20 Mo5 O8 96.14(18) . . ? 
O13 Mo5 O8 149.55(16) . . ? 
O26 Mo5 O18 92.95(17) . . ? 
O20 Mo5 O18 160.33(16) . . ? 
O13 Mo5 O18 79.90(15) . . ? 
O8 Mo5 O18 79.47(15) . . ? 
O26 Mo5 O16 164.53(17) . . ? 
O20 Mo5 O16 88.75(16) . . ? 
O13 Mo5 O16 76.16(14) . . ? 
O8 Mo5 O16 76.21(14) . . ? 
O18 Mo5 O16 71.58(13) . . ? 
O26 Mo5 Mo4 134.97(16) . . ? 
O20 Mo5 Mo4 83.35(14) . . ? 
O13 Mo5 Mo4 33.03(11) . . ? 
O8 Mo5 Mo4 121.68(11) . . ? 
O18 Mo5 Mo4 82.80(10) . . ? 
O16 Mo5 Mo4 45.49(9) . . ? 
O26 Mo5 Mo6 134.19(16) . . ? 
O20 Mo5 Mo6 83.46(13) . . ? 
O13 Mo5 Mo6 121.68(11) . . ? 
O8 Mo5 Mo6 33.08(11) . . ? 
O18 Mo5 Mo6 82.62(10) . . ? 
O16 Mo5 Mo6 45.55(9) . . ? 
Mo4 Mo5 Mo6 89.894(17) . . ? 
O12 Mo6 O3 105.72(19) . . ? 
O12 Mo6 O8 100.96(18) . . ? 
O3 Mo6 O8 99.23(17) . . ? 
O12 Mo6 O5 99.97(17) . . ? 
O3 Mo6 O5 97.07(16) . . ? 
O8 Mo6 O5 148.78(15) . . ? 
O12 Mo6 O19 93.02(17) . . ? 
O3 Mo6 O19 160.41(16) . . ? 
O8 Mo6 O19 82.37(14) . . ? 
O5 Mo6 O19 73.62(14) . . ? 
O12 Mo6 O16 165.08(17) . . ? 
O3 Mo6 O16 89.14(16) . . ? 
O8 Mo6 O16 77.45(14) . . ? 
O5 Mo6 O16 76.37(13) . . ? 
O19 Mo6 O16 72.06(13) . . ? 
O12 Mo6 Mo5 134.22(14) . . ? 
O3 Mo6 Mo5 85.81(13) . . ? 
O8 Mo6 Mo5 33.38(12) . . ? 
O5 Mo6 Mo5 122.85(10) . . ? 
O19 Mo6 Mo5 85.11(9) . . ? 
O16 Mo6 Mo5 46.53(9) . . ? 
O6 V1 O18 106.10(19) . . ? 
O6 V1 O19 99.67(17) . . ? 
O18 V1 O19 97.03(17) . . ? 
O6 V1 O4 99.55(17) . . ? 
O18 V1 O4 97.16(17) . . ? 
O19 V1 O4 151.86(15) . . ? 
O6 V1 O1 93.26(16) . . ? 
O18 V1 O1 160.64(16) . . ? 
O19 V1 O1 78.87(14) . . ? 
O4 V1 O1 79.70(14) . . ? 
O6 V1 O16 170.29(17) . . ? 
O18 V1 O16 83.61(16) . . ? 
O19 V1 O16 78.68(14) . . ? 
O4 V1 O16 78.90(14) . . ? 
O1 V1 O16 77.03(13) . . ? 
O6 V1 Mo3 86.38(14) . . ? 
O18 V1 Mo3 133.30(13) . . ? 
O19 V1 Mo3 125.63(11) . . ? 
O4 V1 Mo3 36.17(10) . . ? 
O1 V1 Mo3 46.77(9) . . ? 
O16 V1 Mo3 86.89(10) . . ? 
O7 V2 O11 105.87(19) . . ? 
O7 V2 O5 99.46(17) . . ? 
O11 V2 O5 97.86(17) . . ? 
O7 V2 O10 99.13(17) . . ? 
O11 V2 O10 97.06(17) . . ? 
O5 V2 O10 151.92(15) . . ? 
O7 V2 O16 93.00(17) . . ? 
O11 V2 O16 161.11(16) . . ? 
O5 V2 O16 79.29(14) . . ? 
O10 V2 O16 78.90(14) . . ? 
O7 V2 O1 169.62(17) . . ? 
O11 V2 O1 84.50(16) . . ? 
O5 V2 O1 79.01(14) . . ? 
O10 V2 O1 78.91(14) . . ? 
O16 V2 O1 76.63(13) . . ? 
V1 O1 V2 103.46(15) . . ? 
V1 O1 Mo1 90.91(13) . . ? 
V2 O1 Mo1 97.82(14) . . ? 
V1 O1 Mo3 89.67(13) . . ? 
V2 O1 Mo3 97.62(14) . . ? 
Mo1 O1 Mo3 163.97(18) . . ? 
V1 O1 Mo2 165.44(18) . . ? 
V2 O1 Mo2 91.07(13) . . ? 
Mo1 O1 Mo2 87.98(12) . . ? 
Mo3 O1 Mo2 87.46(12) . . ? 
Mo6 O3 La2 136.81(19) . . ? 
V1 O4 Mo3 107.99(16) . . ? 
V1 O4 Mo4 108.80(16) . . ? 
Mo3 O4 Mo4 103.23(15) . . ? 
V2 O5 Mo6 108.46(16) . . ? 
V2 O5 Mo1 108.83(16) . . ? 
Mo6 O5 Mo1 102.49(15) . . ? 
V1 O6 La1 133.3(2) . . ? 
V2 O7 La2 133.9(2) . . ? 
Mo6 O8 Mo5 113.53(19) . . ? 
Mo4 O9 La2 135.9(2) . . ? 
V2 O10 Mo4 107.96(17) . . ? 
V2 O10 Mo3 109.49(16) . . ? 
Mo4 O10 Mo3 103.14(16) . . ? 
V2 O11 Mo2 112.65(19) . . ? 
Mo4 O13 Mo5 113.47(18) . . ? 
Mo2 O14 La1 133.9(2) . . ? 
Mo1 O15 Mo2 113.60(18) . . ? 
V2 O16 V1 102.88(15) . . ? 
V2 O16 Mo4 90.28(13) . . ? 
V1 O16 Mo4 98.19(14) . . ? 
V2 O16 Mo6 89.95(13) . . ? 
V1 O16 Mo6 97.96(14) . . ? 
Mo4 O16 Mo6 163.38(18) . . ? 
V2 O16 Mo5 165.72(18) . . ? 
V1 O16 Mo5 91.39(13) . . ? 
Mo4 O16 Mo5 87.77(12) . . ? 
Mo6 O16 Mo5 87.92(13) . . ? 
Mo1 O17 La1 134.72(19) . . ? 
V1 O18 Mo5 113.41(18) . . ? 
V1 O19 Mo1 108.14(17) . . ? 
V1 O19 Mo6 109.38(16) . . ? 
Mo1 O19 Mo6 102.71(15) . . ? 
Mo5 O20 La2 136.0(2) . . ? 
Mo3 O21 Mo2 114.07(19) . . ? 
Mo3 O22 La1 135.44(19) . . ? 
 
loop_ 
 _geom_torsion_atom_site_label_1 
 _geom_torsion_atom_site_label_2 
 _geom_torsion_atom_site_label_3 
 _geom_torsion_atom_site_label_4 
 _geom_torsion 
 _geom_torsion_site_symmetry_1 
 _geom_torsion_site_symmetry_2 
 _geom_torsion_site_symmetry_3 
 _geom_torsion_site_symmetry_4 
 _geom_torsion_publ_flag 
O23 Mo1 Mo2 O2 1.2(3) . . . . ? 
O17 Mo1 Mo2 O2 -108.9(2) . . . . ? 
O15 Mo1 Mo2 O2 4.0(3) . . . . ? 
O19 Mo1 Mo2 O2 155.6(2) . . . . ? 
O5 Mo1 Mo2 O2 88.7(2) . . . . ? 
O1 Mo1 Mo2 O2 158.6(2) . . . . ? 
O23 Mo1 Mo2 O14 108.3(2) . . . . ? 
O17 Mo1 Mo2 O14 -1.84(17) . . . . ? 
O15 Mo1 Mo2 O14 111.1(2) . . . . ? 
O19 Mo1 Mo2 O14 -97.35(18) . . . . ? 
O5 Mo1 Mo2 O14 -164.18(16) . . . . ? 
O1 Mo1 Mo2 O14 -94.35(18) . . . . ? 
O23 Mo1 Mo2 O15 -2.8(3) . . . . ? 
O17 Mo1 Mo2 O15 -113.0(2) . . . . ? 
O19 Mo1 Mo2 O15 151.5(2) . . . . ? 
O5 Mo1 Mo2 O15 84.7(2) . . . . ? 
O1 Mo1 Mo2 O15 154.5(2) . . . . ? 
O23 Mo1 Mo2 O21 -158.7(2) . . . . ? 
O17 Mo1 Mo2 O21 91.16(18) . . . . ? 
O15 Mo1 Mo2 O21 -155.9(2) . . . . ? 
O19 Mo1 Mo2 O21 -4.36(18) . . . . ? 
O5 Mo1 Mo2 O21 -71.19(16) . . . . ? 
O1 Mo1 Mo2 O21 -1.36(18) . . . . ? 
O23 Mo1 Mo2 O11 -85.7(2) . . . . ? 
O17 Mo1 Mo2 O11 164.16(15) . . . . ? 
O15 Mo1 Mo2 O11 -82.9(2) . . . . ? 
O19 Mo1 Mo2 O11 68.64(16) . . . . ? 
O5 Mo1 Mo2 O11 1.81(13) . . . . ? 
O1 Mo1 Mo2 O11 71.65(16) . . . . ? 
O23 Mo1 Mo2 O1 -157.3(2) . . . . ? 
O17 Mo1 Mo2 O1 92.51(17) . . . . ? 
O15 Mo1 Mo2 O1 -154.5(2) . . . . ? 
O19 Mo1 Mo2 O1 -3.01(17) . . . . ? 
O5 Mo1 Mo2 O1 -69.83(15) . . . . ? 
O23 Mo1 Mo2 Mo3 -168.3(2) . . . . ? 
O17 Mo1 Mo2 Mo3 81.56(12) . . . . ? 
O15 Mo1 Mo2 Mo3 -165.5(2) . . . . ? 
O19 Mo1 Mo2 Mo3 -13.95(13) . . . . ? 
O5 Mo1 Mo2 Mo3 -80.78(9) . . . . ? 
O1 Mo1 Mo2 Mo3 -10.95(12) . . . . ? 
O2 Mo2 Mo3 O25 0.8(3) . . . . ? 
O14 Mo2 Mo3 O25 -104.6(2) . . . . ? 
O15 Mo2 Mo3 O25 161.3(2) . . . . ? 
O21 Mo2 Mo3 O25 5.8(3) . . . . ? 
O11 Mo2 Mo3 O25 88.0(2) . . . . ? 
O1 Mo2 Mo3 O25 159.7(2) . . . . ? 
Mo1 Mo2 Mo3 O25 170.5(2) . . . . ? 
O2 Mo2 Mo3 O22 109.1(2) . . . . ? 
O14 Mo2 Mo3 O22 3.63(18) . . . . ? 
O15 Mo2 Mo3 O22 -90.43(18) . . . . ? 
O21 Mo2 Mo3 O22 114.1(2) . . . . ? 
O11 Mo2 Mo3 O22 -163.71(16) . . . . ? 
O1 Mo2 Mo3 O22 -92.03(18) . . . . ? 
Mo1 Mo2 Mo3 O22 -81.19(13) . . . . ? 
O2 Mo2 Mo3 O21 -5.0(3) . . . . ? 
O14 Mo2 Mo3 O21 -110.5(2) . . . . ? 
O15 Mo2 Mo3 O21 155.5(2) . . . . ? 
O11 Mo2 Mo3 O21 82.2(2) . . . . ? 
O1 Mo2 Mo3 O21 153.9(2) . . . . ? 
Mo1 Mo2 Mo3 O21 164.7(2) . . . . ? 
O2 Mo2 Mo3 O4 -155.4(2) . . . . ? 
O14 Mo2 Mo3 O4 99.14(18) . . . . ? 
O15 Mo2 Mo3 O4 5.08(18) . . . . ? 
O21 Mo2 Mo3 O4 -150.4(2) . . . . ? 
O11 Mo2 Mo3 O4 -68.20(16) . . . . ? 
O1 Mo2 Mo3 O4 3.48(17) . . . . ? 
Mo1 Mo2 Mo3 O4 14.32(13) . . . . ? 
O2 Mo2 Mo3 O10 -89.0(2) . . . . ? 
O14 Mo2 Mo3 O10 165.51(17) . . . . ? 
O15 Mo2 Mo3 O10 71.45(16) . . . . ? 
O21 Mo2 Mo3 O10 -84.0(2) . . . . ? 
O11 Mo2 Mo3 O10 -1.83(14) . . . . ? 
O1 Mo2 Mo3 O10 69.85(16) . . . . ? 
Mo1 Mo2 Mo3 O10 80.69(9) . . . . ? 
O2 Mo2 Mo3 O1 -158.9(2) . . . . ? 
O14 Mo2 Mo3 O1 95.66(18) . . . . ? 
O15 Mo2 Mo3 O1 1.60(18) . . . . ? 
O21 Mo2 Mo3 O1 -153.9(2) . . . . ? 
O11 Mo2 Mo3 O1 -71.68(16) . . . . ? 
Mo1 Mo2 Mo3 O1 10.84(12) . . . . ? 
O2 Mo2 Mo3 V1 -168.7(2) . . . . ? 
O14 Mo2 Mo3 V1 85.87(14) . . . . ? 
O15 Mo2 Mo3 V1 -8.18(14) . . . . ? 
O21 Mo2 Mo3 V1 -163.7(2) . . . . ? 
O11 Mo2 Mo3 V1 -81.46(10) . . . . ? 
O1 Mo2 Mo3 V1 -9.79(12) . . . . ? 
Mo1 Mo2 Mo3 V1 1.05(2) . . . . ? 
O24 Mo4 Mo5 O26 0.0(3) . . . . ? 
O9 Mo4 Mo5 O26 109.3(2) . . . . ? 
O13 Mo4 Mo5 O26 -4.4(3) . . . . ? 
O10 Mo4 Mo5 O26 -154.2(2) . . . . ? 
O4 Mo4 Mo5 O26 -88.3(2) . . . . ? 
O16 Mo4 Mo5 O26 -158.2(2) . . . . ? 
O24 Mo4 Mo5 O20 -107.0(2) . . . . ? 
O9 Mo4 Mo5 O20 2.24(18) . . . . ? 
O13 Mo4 Mo5 O20 -111.5(2) . . . . ? 
O10 Mo4 Mo5 O20 98.77(19) . . . . ? 
O4 Mo4 Mo5 O20 164.66(16) . . . . ? 
O16 Mo4 Mo5 O20 94.81(18) . . . . ? 
O24 Mo4 Mo5 O13 4.5(3) . . . . ? 
O9 Mo4 Mo5 O13 113.7(2) . . . . ? 
O10 Mo4 Mo5 O13 -149.8(2) . . . . ? 
O4 Mo4 Mo5 O13 -83.9(2) . . . . ? 
O16 Mo4 Mo5 O13 -153.7(2) . . . . ? 
O24 Mo4 Mo5 O8 159.9(2) . . . . ? 
O9 Mo4 Mo5 O8 -90.88(18) . . . . ? 
O13 Mo4 Mo5 O8 155.4(2) . . . . ? 
O10 Mo4 Mo5 O8 5.64(19) . . . . ? 
O4 Mo4 Mo5 O8 71.54(16) . . . . ? 
O16 Mo4 Mo5 O8 1.69(18) . . . . ? 
O24 Mo4 Mo5 O18 87.0(2) . . . . ? 
O9 Mo4 Mo5 O18 -163.76(15) . . . . ? 
O13 Mo4 Mo5 O18 82.5(2) . . . . ? 
O10 Mo4 Mo5 O18 -67.24(16) . . . . ? 
O4 Mo4 Mo5 O18 -1.34(13) . . . . ? 
O16 Mo4 Mo5 O18 -71.19(16) . . . . ? 
O24 Mo4 Mo5 O16 158.2(2) . . . . ? 
O9 Mo4 Mo5 O16 -92.57(17) . . . . ? 
O13 Mo4 Mo5 O16 153.7(2) . . . . ? 
O10 Mo4 Mo5 O16 3.95(17) . . . . ? 
O4 Mo4 Mo5 O16 69.85(15) . . . . ? 
O24 Mo4 Mo5 Mo6 169.6(2) . . . . ? 
O9 Mo4 Mo5 Mo6 -81.18(12) . . . . ? 
O13 Mo4 Mo5 Mo6 165.1(2) . . . . ? 
O10 Mo4 Mo5 Mo6 15.34(13) . . . . ? 
O4 Mo4 Mo5 Mo6 81.24(9) . . . . ? 
O16 Mo4 Mo5 Mo6 11.39(12) . . . . ? 
O26 Mo5 Mo6 O12 -1.0(3) . . . . ? 
O20 Mo5 Mo6 O12 106.0(2) . . . . ? 
O13 Mo5 Mo6 O12 -161.2(2) . . . . ? 
O8 Mo5 Mo6 O12 -5.9(3) . . . . ? 
O18 Mo5 Mo6 O12 -87.9(2) . . . . ? 
O16 Mo5 Mo6 O12 -159.3(2) . . . . ? 
Mo4 Mo5 Mo6 O12 -170.66(19) . . . . ? 
O26 Mo5 Mo6 O3 -108.9(2) . . . . ? 
O20 Mo5 Mo6 O3 -1.90(18) . . . . ? 
O13 Mo5 Mo6 O3 90.90(18) . . . . ? 
O8 Mo5 Mo6 O3 -113.8(2) . . . . ? 
O18 Mo5 Mo6 O3 164.17(16) . . . . ? 
O16 Mo5 Mo6 O3 92.79(18) . . . . ? 
Mo4 Mo5 Mo6 O3 81.42(12) . . . . ? 
O26 Mo5 Mo6 O8 4.9(3) . . . . ? 
O20 Mo5 Mo6 O8 111.9(2) . . . . ? 
O13 Mo5 Mo6 O8 -155.3(2) . . . . ? 
O18 Mo5 Mo6 O8 -82.0(2) . . . . ? 
O16 Mo5 Mo6 O8 -153.4(2) . . . . ? 
Mo4 Mo5 Mo6 O8 -164.8(2) . . . . ? 
O26 Mo5 Mo6 O5 155.4(2) . . . . ? 
O20 Mo5 Mo6 O5 -97.61(19) . . . . ? 
O13 Mo5 Mo6 O5 -4.82(18) . . . . ? 
O8 Mo5 Mo6 O5 150.5(2) . . . . ? 
O18 Mo5 Mo6 O5 68.46(16) . . . . ? 
O16 Mo5 Mo6 O5 -2.92(17) . . . . ? 
Mo4 Mo5 Mo6 O5 -14.30(13) . . . . ? 
O26 Mo5 Mo6 O19 88.5(2) . . . . ? 
O20 Mo5 Mo6 O19 -164.52(17) . . . . ? 
O13 Mo5 Mo6 O19 -71.73(16) . . . . ? 
O8 Mo5 Mo6 O19 83.6(2) . . . . ? 
O18 Mo5 Mo6 O19 1.55(13) . . . . ? 
O16 Mo5 Mo6 O19 -69.83(16) . . . . ? 
Mo4 Mo5 Mo6 O19 -81.21(9) . . . . ? 
O26 Mo5 Mo6 O16 158.3(2) . . . . ? 
O20 Mo5 Mo6 O16 -94.69(19) . . . . ? 
O13 Mo5 Mo6 O16 -1.90(18) . . . . ? 
O8 Mo5 Mo6 O16 153.4(2) . . . . ? 
O18 Mo5 Mo6 O16 71.38(16) . . . . ? 
Mo4 Mo5 Mo6 O16 -11.38(12) . . . . ? 
O25 Mo3 V1 O6 102.9(2) . . . . ? 
O22 Mo3 V1 O6 -0.83(18) . . . . ? 
O21 Mo3 V1 O6 -97.94(19) . . . . ? 
O4 Mo3 V1 O6 111.6(2) . . . . ? 
O10 Mo3 V1 O6 -172.59(16) . . . . ? 
O1 Mo3 V1 O6 -97.92(19) . . . . ? 
Mo2 Mo3 V1 O6 -87.56(13) . . . . ? 
O25 Mo3 V1 O18 -5.9(3) . . . . ? 
O22 Mo3 V1 O18 -109.6(2) . . . . ? 
O21 Mo3 V1 O18 153.3(2) . . . . ? 
O4 Mo3 V1 O18 2.8(2) . . . . ? 
O10 Mo3 V1 O18 78.6(2) . . . . ? 
O1 Mo3 V1 O18 153.3(2) . . . . ? 
Mo2 Mo3 V1 O18 163.65(18) . . . . ? 
O25 Mo3 V1 O19 -157.8(2) . . . . ? 
O22 Mo3 V1 O19 98.48(19) . . . . ? 
O21 Mo3 V1 O19 1.37(19) . . . . ? 
O4 Mo3 V1 O19 -149.1(2) . . . . ? 
O10 Mo3 V1 O19 -73.29(16) . . . . ? 
O1 Mo3 V1 O19 1.39(18) . . . . ? 
Mo2 Mo3 V1 O19 11.74(14) . . . . ? 
O25 Mo3 V1 O4 -8.7(3) . . . . ? 
O22 Mo3 V1 O4 -112.4(2) . . . . ? 
O21 Mo3 V1 O4 150.4(2) . . . . ? 
O10 Mo3 V1 O4 75.8(2) . . . . ? 
O1 Mo3 V1 O4 150.5(2) . . . . ? 
Mo2 Mo3 V1 O4 160.82(18) . . . . ? 
O25 Mo3 V1 O1 -159.2(2) . . . . ? 
O22 Mo3 V1 O1 97.09(18) . . . . ? 
O21 Mo3 V1 O1 -0.02(18) . . . . ? 
O4 Mo3 V1 O1 -150.5(2) . . . . ? 
O10 Mo3 V1 O1 -74.68(16) . . . . ? 
Mo2 Mo3 V1 O1 10.35(13) . . . . ? 
O25 Mo3 V1 O16 -84.1(2) . . . . ? 
O22 Mo3 V1 O16 172.17(16) . . . . ? 
O21 Mo3 V1 O16 75.07(16) . . . . ? 
O4 Mo3 V1 O16 -75.4(2) . . . . ? 
O10 Mo3 V1 O16 0.41(13) . . . . ? 
O1 Mo3 V1 O16 75.09(16) . . . . ? 
Mo2 Mo3 V1 O16 85.44(9) . . . . ? 
O6 V1 O1 V2 179.69(17) . . . . ? 
O18 V1 O1 V2 -1.7(6) . . . . ? 
O19 V1 O1 V2 -81.09(16) . . . . ? 
O4 V1 O1 V2 80.56(16) . . . . ? 
O16 V1 O1 V2 -0.29(13) . . . . ? 
Mo3 V1 O1 V2 97.76(16) . . . . ? 
O6 V1 O1 Mo1 -82.05(16) . . . . ? 
O18 V1 O1 Mo1 96.6(5) . . . . ? 
O19 V1 O1 Mo1 17.17(13) . . . . ? 
O4 V1 O1 Mo1 178.82(15) . . . . ? 
O16 V1 O1 Mo1 97.97(14) . . . . ? 
Mo3 V1 O1 Mo1 -163.98(18) . . . . ? 
O6 V1 O1 Mo3 81.93(16) . . . . ? 
O18 V1 O1 Mo3 -99.4(5) . . . . ? 
O19 V1 O1 Mo3 -178.85(15) . . . . ? 
O4 V1 O1 Mo3 -17.20(13) . . . . ? 
O16 V1 O1 Mo3 -98.05(13) . . . . ? 
O6 V1 O1 Mo2 3.4(7) . . . . ? 
O18 V1 O1 Mo2 -178.0(6) . . . . ? 
O19 V1 O1 Mo2 102.6(7) . . . . ? 
O4 V1 O1 Mo2 -95.7(7) . . . . ? 
O16 V1 O1 Mo2 -176.6(7) . . . . ? 
Mo3 V1 O1 Mo2 -78.5(7) . . . . ? 
O7 V2 O1 V1 -0.7(10) . . . . ? 
O11 V2 O1 V1 -179.11(18) . . . . ? 
O5 V2 O1 V1 81.76(16) . . . . ? 
O10 V2 O1 V1 -80.78(16) . . . . ? 
O16 V2 O1 V1 0.30(14) . . . . ? 
O7 V2 O1 Mo1 -93.5(9) . . . . ? 
O11 V2 O1 Mo1 88.07(16) . . . . ? 
O5 V2 O1 Mo1 -11.06(14) . . . . ? 
O10 V2 O1 Mo1 -173.61(16) . . . . ? 
O16 V2 O1 Mo1 -92.53(14) . . . . ? 
O7 V2 O1 Mo3 90.8(9) . . . . ? 
O11 V2 O1 Mo3 -87.61(16) . . . . ? 
O5 V2 O1 Mo3 173.26(16) . . . . ? 
O10 V2 O1 Mo3 10.71(14) . . . . ? 
O16 V2 O1 Mo3 91.79(14) . . . . ? 
O7 V2 O1 Mo2 178.4(9) . . . . ? 
O11 V2 O1 Mo2 -0.04(15) . . . . ? 
O5 V2 O1 Mo2 -99.17(14) . . . . ? 
O10 V2 O1 Mo2 98.28(14) . . . . ? 
O16 V2 O1 Mo2 179.37(15) . . . . ? 
O23 Mo1 O1 V1 -90.9(6) . . . . ? 
O17 Mo1 O1 V1 78.89(16) . . . . ? 
O15 Mo1 O1 V1 179.48(16) . . . . ? 
O19 Mo1 O1 V1 -17.13(13) . . . . ? 
O5 Mo1 O1 V1 -93.83(14) . . . . ? 
Mo2 Mo1 O1 V1 165.48(18) . . . . ? 
O23 Mo1 O1 V2 12.8(7) . . . . ? 
O17 Mo1 O1 V2 -177.40(16) . . . . ? 
O15 Mo1 O1 V2 -76.80(16) . . . . ? 
O19 Mo1 O1 V2 86.59(15) . . . . ? 
O5 Mo1 O1 V2 9.89(12) . . . . ? 
Mo2 Mo1 O1 V2 -90.80(14) . . . . ? 
O23 Mo1 O1 Mo3 177.1(6) . . . . ? 
O17 Mo1 O1 Mo3 -13.1(6) . . . . ? 
O15 Mo1 O1 Mo3 87.5(6) . . . . ? 
O19 Mo1 O1 Mo3 -109.1(6) . . . . ? 
O5 Mo1 O1 Mo3 174.2(7) . . . . ? 
Mo2 Mo1 O1 Mo3 73.5(6) . . . . ? 
O23 Mo1 O1 Mo2 103.6(6) . . . . ? 
O17 Mo1 O1 Mo2 -86.59(15) . . . . ? 
O15 Mo1 O1 Mo2 14.00(14) . . . . ? 
O19 Mo1 O1 Mo2 177.39(15) . . . . ? 
O5 Mo1 O1 Mo2 100.70(13) . . . . ? 
O25 Mo3 O1 V1 90.6(7) . . . . ? 
O22 Mo3 O1 V1 -79.52(16) . . . . ? 
O21 Mo3 O1 V1 179.98(16) . . . . ? 
O4 Mo3 O1 V1 17.28(13) . . . . ? 
O10 Mo3 O1 V1 93.87(14) . . . . ? 
Mo2 Mo3 O1 V1 -165.72(18) . . . . ? 
O25 Mo3 O1 V2 -12.9(7) . . . . ? 
O22 Mo3 O1 V2 176.94(16) . . . . ? 
O21 Mo3 O1 V2 76.44(16) . . . . ? 
O4 Mo3 O1 V2 -86.26(15) . . . . ? 
O10 Mo3 O1 V2 -9.66(12) . . . . ? 
V1 Mo3 O1 V2 -103.54(16) . . . . ? 
Mo2 Mo3 O1 V2 90.74(14) . . . . ? 
O25 Mo3 O1 Mo1 -177.3(6) . . . . ? 
O22 Mo3 O1 Mo1 12.6(6) . . . . ? 
O21 Mo3 O1 Mo1 -87.9(6) . . . . ? 
O4 Mo3 O1 Mo1 109.4(6) . . . . ? 
O10 Mo3 O1 Mo1 -174.0(7) . . . . ? 
V1 Mo3 O1 Mo1 92.1(6) . . . . ? 
Mo2 Mo3 O1 Mo1 -73.6(6) . . . . ? 
O25 Mo3 O1 Mo2 -103.7(6) . . . . ? 
O22 Mo3 O1 Mo2 86.20(15) . . . . ? 
O21 Mo3 O1 Mo2 -14.30(14) . . . . ? 
O4 Mo3 O1 Mo2 -177.00(15) . . . . ? 
O10 Mo3 O1 Mo2 -100.41(14) . . . . ? 
V1 Mo3 O1 Mo2 165.72(18) . . . . ? 
O2 Mo2 O1 V1 175.1(7) . . . . ? 
O14 Mo2 O1 V1 -2.5(7) . . . . ? 
O15 Mo2 O1 V1 -99.8(7) . . . . ? 
O21 Mo2 O1 V1 93.0(7) . . . . ? 
O11 Mo2 O1 V1 176.4(7) . . . . ? 
Mo1 Mo2 O1 V1 -85.8(7) . . . . ? 
Mo3 Mo2 O1 V1 78.8(7) . . . . ? 
O2 Mo2 O1 V2 -1.3(7) . . . . ? 
O14 Mo2 O1 V2 -178.93(16) . . . . ? 
O15 Mo2 O1 V2 83.83(15) . . . . ? 
O21 Mo2 O1 V2 -83.40(15) . . . . ? 
O11 Mo2 O1 V2 0.03(12) . . . . ? 
Mo1 Mo2 O1 V2 97.79(14) . . . . ? 
Mo3 Mo2 O1 V2 -97.58(14) . . . . ? 
O2 Mo2 O1 Mo1 -99.1(7) . . . . ? 
O14 Mo2 O1 Mo1 83.28(16) . . . . ? 
O15 Mo2 O1 Mo1 -13.96(13) . . . . ? 
O21 Mo2 O1 Mo1 178.81(16) . . . . ? 
O11 Mo2 O1 Mo1 -97.76(14) . . . . ? 
Mo3 Mo2 O1 Mo1 164.63(17) . . . . ? 
O2 Mo2 O1 Mo3 96.3(7) . . . . ? 
O14 Mo2 O1 Mo3 -81.35(16) . . . . ? 
O15 Mo2 O1 Mo3 -178.59(16) . . . . ? 
O21 Mo2 O1 Mo3 14.18(13) . . . . ? 
O11 Mo2 O1 Mo3 97.61(14) . . . . ? 
Mo1 Mo2 O1 Mo3 -164.63(17) . . . . ? 
O12 Mo6 O3 La2 -178.1(3) . . . . ? 
O8 Mo6 O3 La2 -73.9(3) . . . . ? 
O5 Mo6 O3 La2 79.4(3) . . . . ? 
O19 Mo6 O3 La2 19.3(7) . . . . ? 
O16 Mo6 O3 La2 3.3(3) . . . . ? 
Mo5 Mo6 O3 La2 -43.2(3) . . . . ? 
O7W La2 O3 Mo6 -143.6(3) . . . . ? 
O6W La2 O3 Mo6 173.6(2) . . . . ? 
O9 La2 O3 Mo6 -3.8(3) . . . . ? 
O9W La2 O3 Mo6 -80.9(4) . . . . ? 
O10W La2 O3 Mo6 128.3(3) . . . . ? 
O8W La2 O3 Mo6 77.1(3) . . . . ? 
O20 La2 O3 Mo6 55.8(3) . . . . ? 
O7 La2 O3 Mo6 -59.7(3) . . . . ? 
O6 V1 O4 Mo3 -70.2(2) . . . . ? 
O18 V1 O4 Mo3 -177.93(18) . . . . ? 
O19 V1 O4 Mo3 62.3(4) . . . . ? 
O1 V1 O4 Mo3 21.41(16) . . . . ? 
O16 V1 O4 Mo3 100.06(17) . . . . ? 
O6 V1 O4 Mo4 178.40(17) . . . . ? 
O18 V1 O4 Mo4 70.68(19) . . . . ? 
O19 V1 O4 Mo4 -49.1(4) . . . . ? 
O1 V1 O4 Mo4 -89.99(16) . . . . ? 
O16 V1 O4 Mo4 -11.34(14) . . . . ? 
Mo3 V1 O4 Mo4 -111.4(2) . . . . ? 
O25 Mo3 O4 V1 173.74(19) . . . . ? 
O22 Mo3 O4 V1 67.2(2) . . . . ? 
O21 Mo3 O4 V1 -54.6(4) . . . . ? 
O10 Mo3 O4 V1 -95.41(18) . . . . ? 
O1 Mo3 O4 V1 -20.46(15) . . . . ? 
Mo2 Mo3 O4 V1 -23.1(2) . . . . ? 
O25 Mo3 O4 Mo4 -71.14(19) . . . . ? 
O22 Mo3 O4 Mo4 -177.73(16) . . . . ? 
O21 Mo3 O4 Mo4 60.5(3) . . . . ? 
O10 Mo3 O4 Mo4 19.71(13) . . . . ? 
O1 Mo3 O4 Mo4 94.66(15) . . . . ? 
V1 Mo3 O4 Mo4 115.1(2) . . . . ? 
Mo2 Mo3 O4 Mo4 92.05(13) . . . . ? 
O24 Mo4 O4 V1 -170.21(19) . . . . ? 
O9 Mo4 O4 V1 33.0(6) . . . . ? 
O13 Mo4 O4 V1 -68.10(18) . . . . ? 
O10 Mo4 O4 V1 92.18(18) . . . . ? 
O16 Mo4 O4 V1 11.41(15) . . . . ? 
Mo5 Mo4 O4 V1 -34.50(13) . . . . ? 
O24 Mo4 O4 Mo3 75.25(19) . . . . ? 
O9 Mo4 O4 Mo3 -81.5(5) . . . . ? 
O13 Mo4 O4 Mo3 177.36(18) . . . . ? 
O10 Mo4 O4 Mo3 -22.36(15) . . . . ? 
O16 Mo4 O4 Mo3 -103.12(16) . . . . ? 
Mo5 Mo4 O4 Mo3 -149.04(13) . . . . ? 
O7 V2 O5 Mo6 70.6(2) . . . . ? 
O11 V2 O5 Mo6 178.26(18) . . . . ? 
O10 V2 O5 Mo6 -60.2(4) . . . . ? 
O16 V2 O5 Mo6 -20.66(16) . . . . ? 
O1 V2 O5 Mo6 -98.94(17) . . . . ? 
O7 V2 O5 Mo1 -178.60(17) . . . . ? 
O11 V2 O5 Mo1 -70.96(19) . . . . ? 
O10 V2 O5 Mo1 50.5(4) . . . . ? 
O16 V2 O5 Mo1 90.12(16) . . . . ? 
O1 V2 O5 Mo1 11.83(14) . . . . ? 
O12 Mo6 O5 V2 -174.76(19) . . . . ? 
O3 Mo6 O5 V2 -67.4(2) . . . . ? 
O8 Mo6 O5 V2 53.7(4) . . . . ? 
O19 Mo6 O5 V2 95.01(18) . . . . ? 
O16 Mo6 O5 V2 20.02(16) . . . . ? 
Mo5 Mo6 O5 V2 22.2(2) . . . . ? 
O12 Mo6 O5 Mo1 70.24(19) . . . . ? 
O3 Mo6 O5 Mo1 177.65(16) . . . . ? 
O8 Mo6 O5 Mo1 -61.3(3) . . . . ? 
O19 Mo6 O5 Mo1 -19.99(13) . . . . ? 
O16 Mo6 O5 Mo1 -94.97(15) . . . . ? 
Mo5 Mo6 O5 Mo1 -92.79(13) . . . . ? 
O23 Mo1 O5 V2 168.9(2) . . . . ? 
O17 Mo1 O5 V2 -34.9(6) . . . . ? 
O15 Mo1 O5 V2 67.55(18) . . . . ? 
O19 Mo1 O5 V2 -92.08(18) . . . . ? 
O1 Mo1 O5 V2 -11.92(15) . . . . ? 
Mo2 Mo1 O5 V2 34.04(13) . . . . ? 
O23 Mo1 O5 Mo6 -76.38(19) . . . . ? 
O17 Mo1 O5 Mo6 79.8(5) . . . . ? 
O15 Mo1 O5 Mo6 -177.73(17) . . . . ? 
O19 Mo1 O5 Mo6 22.64(15) . . . . ? 
O1 Mo1 O5 Mo6 102.80(16) . . . . ? 
Mo2 Mo1 O5 Mo6 148.77(13) . . . . ? 
O18 V1 O6 La1 -178.7(2) . . . . ? 
O19 V1 O6 La1 -78.4(3) . . . . ? 
O4 V1 O6 La1 80.9(3) . . . . ? 
O1 V1 O6 La1 0.8(3) . . . . ? 
O16 V1 O6 La1 1.0(12) . . . . ? 
Mo3 V1 O6 La1 47.1(2) . . . . ? 
O1W La1 O6 V1 135.2(3) . . . . ? 
O5W La1 O6 V1 -141.4(3) . . . . ? 
O17 La1 O6 V1 59.2(3) . . . . ? 
O3W La1 O6 V1 75.7(3) . . . . ? 
O22 La1 O6 V1 -61.0(3) . . . . ? 
O2W La1 O6 V1 -80.8(3) . . . . ? 
O4W La1 O6 V1 -179.9(2) . . . . ? 
O14 La1 O6 V1 -2.7(3) . . . . ? 
O11 V2 O7 La2 -179.9(2) . . . . ? 
O5 V2 O7 La2 -78.9(3) . . . . ? 
O10 V2 O7 La2 80.0(3) . . . . ? 
O16 V2 O7 La2 0.8(3) . . . . ? 
O1 V2 O7 La2 1.7(11) . . . . ? 
O7W La2 O7 V2 131.1(3) . . . . ? 
O6W La2 O7 V2 179.0(2) . . . . ? 
O9 La2 O7 V2 -60.4(3) . . . . ? 
O9W La2 O7 V2 -135.2(3) . . . . ? 
O3 La2 O7 V2 58.3(3) . . . . ? 
O10W La2 O7 V2 69.8(3) . . . . ? 
O8W La2 O7 V2 -73.3(3) . . . . ? 
O20 La2 O7 V2 -0.7(3) . . . . ? 
O12 Mo6 O8 Mo5 175.7(2) . . . . ? 
O3 Mo6 O8 Mo5 67.6(2) . . . . ? 
O5 Mo6 O8 Mo5 -53.0(4) . . . . ? 
O19 Mo6 O8 Mo5 -92.68(19) . . . . ? 
O16 Mo6 O8 Mo5 -19.45(18) . . . . ? 
O26 Mo5 O8 Mo6 -176.4(2) . . . . ? 
O20 Mo5 O8 Mo6 -68.0(2) . . . . ? 
O13 Mo5 O8 Mo6 44.6(4) . . . . ? 
O18 Mo5 O8 Mo6 92.6(2) . . . . ? 
O16 Mo5 O8 Mo6 19.22(17) . . . . ? 
Mo4 Mo5 O8 Mo6 18.0(2) . . . . ? 
O24 Mo4 O9 La2 177.9(3) . . . . ? 
O13 Mo4 O9 La2 71.9(3) . . . . ? 
O10 Mo4 O9 La2 -81.9(3) . . . . ? 
O4 Mo4 O9 La2 -26.2(7) . . . . ? 
O16 Mo4 O9 La2 -5.7(3) . . . . ? 
Mo5 Mo4 O9 La2 41.0(2) . . . . ? 
O7W La2 O9 Mo4 80.1(3) . . . . ? 
O6W La2 O9 Mo4 -171.7(2) . . . . ? 
O9W La2 O9 Mo4 145.1(3) . . . . ? 
O3 La2 O9 Mo4 5.7(3) . . . . ? 
O10W La2 O9 Mo4 -72.5(3) . . . . ? 
O8W La2 O9 Mo4 -126.7(3) . . . . ? 
O20 La2 O9 Mo4 -53.2(3) . . . . ? 
O7 La2 O9 Mo4 62.1(3) . . . . ? 
O7 V2 O10 Mo4 -69.7(2) . . . . ? 
O11 V2 O10 Mo4 -177.12(18) . . . . ? 
O5 V2 O10 Mo4 61.2(4) . . . . ? 
O16 V2 O10 Mo4 21.57(16) . . . . ? 
O1 V2 O10 Mo4 99.93(18) . . . . ? 
O7 V2 O10 Mo3 178.68(18) . . . . ? 
O11 V2 O10 Mo3 71.28(19) . . . . ? 
O5 V2 O10 Mo3 -50.4(4) . . . . ? 
O16 V2 O10 Mo3 -90.03(17) . . . . ? 
O1 V2 O10 Mo3 -11.67(15) . . . . ? 
O24 Mo4 O10 V2 173.91(19) . . . . ? 
O9 Mo4 O10 V2 67.4(2) . . . . ? 
O13 Mo4 O10 V2 -56.2(4) . . . . ? 
O4 Mo4 O10 V2 -96.24(18) . . . . ? 
O16 Mo4 O10 V2 -20.98(16) . . . . ? 
Mo5 Mo4 O10 V2 -23.9(2) . . . . ? 
O24 Mo4 O10 Mo3 -70.25(19) . . . . ? 
O9 Mo4 O10 Mo3 -176.81(16) . . . . ? 
O13 Mo4 O10 Mo3 59.6(3) . . . . ? 
O4 Mo4 O10 Mo3 19.60(13) . . . . ? 
O16 Mo4 O10 Mo3 94.85(15) . . . . ? 
Mo5 Mo4 O10 Mo3 91.89(14) . . . . ? 
O25 Mo3 O10 V2 -169.2(2) . . . . ? 
O22 Mo3 O10 V2 31.4(5) . . . . ? 
O21 Mo3 O10 V2 -67.71(18) . . . . ? 
O4 Mo3 O10 V2 92.34(18) . . . . ? 
O1 Mo3 O10 V2 11.64(15) . . . . ? 
V1 Mo3 O10 V2 55.99(14) . . . . ? 
Mo2 Mo3 O10 V2 -34.36(14) . . . . ? 
O25 Mo3 O10 Mo4 76.08(19) . . . . ? 
O22 Mo3 O10 Mo4 -83.4(5) . . . . ? 
O21 Mo3 O10 Mo4 177.55(18) . . . . ? 
O4 Mo3 O10 Mo4 -22.41(15) . . . . ? 
O1 Mo3 O10 Mo4 -103.10(17) . . . . ? 
V1 Mo3 O10 Mo4 -58.75(12) . . . . ? 
Mo2 Mo3 O10 Mo4 -149.10(14) . . . . ? 
O7 V2 O11 Mo2 -179.66(18) . . . . ? 
O5 V2 O11 Mo2 78.1(2) . . . . ? 
O10 V2 O11 Mo2 -78.0(2) . . . . ? 
O16 V2 O11 Mo2 -1.7(6) . . . . ? 
O1 V2 O11 Mo2 0.04(18) . . . . ? 
O2 Mo2 O11 V2 179.6(2) . . . . ? 
O14 Mo2 O11 V2 3.2(6) . . . . ? 
O15 Mo2 O11 V2 -78.5(2) . . . . ? 
O21 Mo2 O11 V2 78.7(2) . . . . ? 
O1 Mo2 O11 V2 -0.04(17) . . . . ? 
Mo1 Mo2 O11 V2 -45.20(17) . . . . ? 
Mo3 Mo2 O11 V2 45.69(17) . . . . ? 
O24 Mo4 O13 Mo5 -176.8(2) . . . . ? 
O9 Mo4 O13 Mo5 -68.5(2) . . . . ? 
O10 Mo4 O13 Mo5 54.3(4) . . . . ? 
O4 Mo4 O13 Mo5 92.5(2) . . . . ? 
O16 Mo4 O13 Mo5 19.27(18) . . . . ? 
O26 Mo5 O13 Mo4 176.8(2) . . . . ? 
O20 Mo5 O13 Mo4 68.3(2) . . . . ? 
O8 Mo5 O13 Mo4 -44.3(4) . . . . ? 
O18 Mo5 O13 Mo4 -92.3(2) . . . . ? 
O16 Mo5 O13 Mo4 -18.98(18) . . . . ? 
Mo6 Mo5 O13 Mo4 -17.6(2) . . . . ? 
O2 Mo2 O14 La1 178.2(3) . . . . ? 
O15 Mo2 O14 La1 73.3(3) . . . . ? 
O21 Mo2 O14 La1 -78.5(3) . . . . ? 
O11 Mo2 O14 La1 -5.6(7) . . . . ? 
O1 Mo2 O14 La1 -2.5(3) . . . . ? 
Mo1 Mo2 O14 La1 42.6(2) . . . . ? 
Mo3 Mo2 O14 La1 -48.0(2) . . . . ? 
O1W La1 O14 Mo2 -79.9(3) . . . . ? 
O5W La1 O14 Mo2 87.3(3) . . . . ? 
O17 La1 O14 Mo2 -55.4(3) . . . . ? 
O3W La1 O14 Mo2 -131.3(3) . . . . ? 
O22 La1 O14 Mo2 60.6(3) . . . . ? 
O2W La1 O14 Mo2 134.8(3) . . . . ? 
O4W La1 O14 Mo2 -178.4(2) . . . . ? 
O6 La1 O14 Mo2 4.0(3) . . . . ? 
O23 Mo1 O15 Mo2 178.0(2) . . . . ? 
O17 Mo1 O15 Mo2 69.3(2) . . . . ? 
O19 Mo1 O15 Mo2 -51.4(4) . . . . ? 
O5 Mo1 O15 Mo2 -91.89(19) . . . . ? 
O1 Mo1 O15 Mo2 -18.70(18) . . . . ? 
O2 Mo2 O15 Mo1 -177.1(2) . . . . ? 
O14 Mo2 O15 Mo1 -69.4(2) . . . . ? 
O21 Mo2 O15 Mo1 43.3(4) . . . . ? 
O11 Mo2 O15 Mo1 91.9(2) . . . . ? 
O1 Mo2 O15 Mo1 18.32(17) . . . . ? 
Mo3 Mo2 O15 Mo1 17.1(2) . . . . ? 
O7 V2 O16 V1 179.53(17) . . . . ? 
O11 V2 O16 V1 1.5(6) . . . . ? 
O5 V2 O16 V1 -81.40(16) . . . . ? 
O10 V2 O16 V1 80.80(16) . . . . ? 
O1 V2 O16 V1 -0.29(13) . . . . ? 
O7 V2 O16 Mo4 81.06(16) . . . . ? 
O11 V2 O16 Mo4 -96.9(5) . . . . ? 
O5 V2 O16 Mo4 -179.87(15) . . . . ? 
O10 V2 O16 Mo4 -17.67(13) . . . . ? 
O1 V2 O16 Mo4 -98.76(14) . . . . ? 
O7 V2 O16 Mo6 -82.32(16) . . . . ? 
O11 V2 O16 Mo6 99.7(5) . . . . ? 
O5 V2 O16 Mo6 16.75(13) . . . . ? 
O10 V2 O16 Mo6 178.96(15) . . . . ? 
O1 V2 O16 Mo6 97.86(13) . . . . ? 
O7 V2 O16 Mo5 -1.0(7) . . . . ? 
O11 V2 O16 Mo5 -178.9(6) . . . . ? 
O5 V2 O16 Mo5 98.1(7) . . . . ? 
O10 V2 O16 Mo5 -99.7(7) . . . . ? 
O1 V2 O16 Mo5 179.2(8) . . . . ? 
O6 V1 O16 V2 0.2(11) . . . . ? 
O18 V1 O16 V2 179.84(18) . . . . ? 
O19 V1 O16 V2 81.33(16) . . . . ? 
O4 V1 O16 V2 -81.55(16) . . . . ? 
O1 V1 O16 V2 0.30(14) . . . . ? 
Mo3 V1 O16 V2 -45.96(12) . . . . ? 
O6 V1 O16 Mo4 92.3(10) . . . . ? 
O18 V1 O16 Mo4 -87.98(17) . . . . ? 
O19 V1 O16 Mo4 173.50(16) . . . . ? 
O4 V1 O16 Mo4 10.63(14) . . . . ? 
O1 V1 O16 Mo4 92.47(14) . . . . ? 
Mo3 V1 O16 Mo4 46.22(10) . . . . ? 
O6 V1 O16 Mo6 -91.6(10) . . . . ? 
O18 V1 O16 Mo6 88.06(16) . . . . ? 
O19 V1 O16 Mo6 -10.46(14) . . . . ? 
O4 V1 O16 Mo6 -173.33(16) . . . . ? 
O1 V1 O16 Mo6 -91.49(14) . . . . ? 
Mo3 V1 O16 Mo6 -137.74(11) . . . . ? 
O6 V1 O16 Mo5 -179.7(9) . . . . ? 
O18 V1 O16 Mo5 -0.04(15) . . . . ? 
O19 V1 O16 Mo5 -98.55(14) . . . . ? 
O4 V1 O16 Mo5 98.57(14) . . . . ? 
O1 V1 O16 Mo5 -179.58(15) . . . . ? 
Mo3 V1 O16 Mo5 134.16(9) . . . . ? 
O24 Mo4 O16 V2 87.5(6) . . . . ? 
O9 Mo4 O16 V2 -79.57(16) . . . . ? 
O13 Mo4 O16 V2 179.66(16) . . . . ? 
O10 Mo4 O16 V2 17.56(13) . . . . ? 
O4 Mo4 O16 V2 93.53(14) . . . . ? 
Mo5 Mo4 O16 V2 -165.85(18) . . . . ? 
O24 Mo4 O16 V1 -15.5(7) . . . . ? 
O9 Mo4 O16 V1 177.38(16) . . . . ? 
O13 Mo4 O16 V1 76.61(16) . . . . ? 
O10 Mo4 O16 V1 -85.50(15) . . . . ? 
O4 Mo4 O16 V1 -9.53(12) . . . . ? 
Mo5 Mo4 O16 V1 91.09(14) . . . . ? 
O24 Mo4 O16 Mo6 178.3(6) . . . . ? 
O9 Mo4 O16 Mo6 11.2(6) . . . . ? 
O13 Mo4 O16 Mo6 -89.6(6) . . . . ? 
O10 Mo4 O16 Mo6 108.3(6) . . . . ? 
O4 Mo4 O16 Mo6 -175.7(6) . . . . ? 
Mo5 Mo4 O16 Mo6 -75.1(6) . . . . ? 
O24 Mo4 O16 Mo5 -106.6(6) . . . . ? 
O9 Mo4 O16 Mo5 86.29(15) . . . . ? 
O13 Mo4 O16 Mo5 -14.48(14) . . . . ? 
O10 Mo4 O16 Mo5 -176.59(15) . . . . ? 
O4 Mo4 O16 Mo5 -100.62(13) . . . . ? 
O12 Mo6 O16 V2 -94.0(6) . . . . ? 
O3 Mo6 O16 V2 80.84(16) . . . . ? 
O8 Mo6 O16 V2 -179.50(16) . . . . ? 
O5 Mo6 O16 V2 -16.64(13) . . . . ? 
O19 Mo6 O16 V2 -93.56(14) . . . . ? 
Mo5 Mo6 O16 V2 165.88(18) . . . . ? 
O12 Mo6 O16 V1 9.0(7) . . . . ? 
O3 Mo6 O16 V1 -176.15(16) . . . . ? 
O8 Mo6 O16 V1 -76.50(16) . . . . ? 
O5 Mo6 O16 V1 86.36(15) . . . . ? 
O19 Mo6 O16 V1 9.44(12) . . . . ? 
Mo5 Mo6 O16 V1 -91.12(14) . . . . ? 
O12 Mo6 O16 Mo4 175.1(6) . . . . ? 
O3 Mo6 O16 Mo4 -10.0(6) . . . . ? 
O8 Mo6 O16 Mo4 89.7(6) . . . . ? 
O5 Mo6 O16 Mo4 -107.5(6) . . . . ? 
O19 Mo6 O16 Mo4 175.6(6) . . . . ? 
Mo5 Mo6 O16 Mo4 75.1(6) . . . . ? 
O12 Mo6 O16 Mo5 100.1(6) . . . . ? 
O3 Mo6 O16 Mo5 -85.04(15) . . . . ? 
O8 Mo6 O16 Mo5 14.62(14) . . . . ? 
O5 Mo6 O16 Mo5 177.48(15) . . . . ? 
O19 Mo6 O16 Mo5 100.56(14) . . . . ? 
O26 Mo5 O16 V2 -178.3(7) . . . . ? 
O20 Mo5 O16 V2 0.4(7) . . . . ? 
O13 Mo5 O16 V2 96.7(7) . . . . ? 
O8 Mo5 O16 V2 -96.2(7) . . . . ? 
O18 Mo5 O16 V2 -179.5(8) . . . . ? 
Mo4 Mo5 O16 V2 82.3(7) . . . . ? 
Mo6 Mo5 O16 V2 -81.6(7) . . . . ? 
O26 Mo5 O16 V1 1.3(7) . . . . ? 
O20 Mo5 O16 V1 179.97(17) . . . . ? 
O13 Mo5 O16 V1 -83.75(15) . . . . ? 
O8 Mo5 O16 V1 83.34(15) . . . . ? 
O18 Mo5 O16 V1 0.03(12) . . . . ? 
Mo4 Mo5 O16 V1 -98.14(14) . . . . ? 
Mo6 Mo5 O16 V1 97.91(14) . . . . ? 
O26 Mo5 O16 Mo4 99.4(7) . . . . ? 
O20 Mo5 O16 Mo4 -81.89(16) . . . . ? 
O13 Mo5 O16 Mo4 14.40(14) . . . . ? 
O8 Mo5 O16 Mo4 -178.52(16) . . . . ? 
O18 Mo5 O16 Mo4 98.18(14) . . . . ? 
Mo6 Mo5 O16 Mo4 -163.94(17) . . . . ? 
O26 Mo5 O16 Mo6 -96.6(7) . . . . ? 
O20 Mo5 O16 Mo6 82.05(16) . . . . ? 
O13 Mo5 O16 Mo6 178.34(16) . . . . ? 
O8 Mo5 O16 Mo6 -14.58(13) . . . . ? 
O18 Mo5 O16 Mo6 -97.88(14) . . . . ? 
Mo4 Mo5 O16 Mo6 163.94(17) . . . . ? 
O23 Mo1 O17 La1 -176.4(3) . . . . ? 
O15 Mo1 O17 La1 -71.2(3) . . . . ? 
O19 Mo1 O17 La1 82.4(3) . . . . ? 
O5 Mo1 O17 La1 28.4(7) . . . . ? 
O1 Mo1 O17 La1 6.5(3) . . . . ? 
Mo2 Mo1 O17 La1 -40.2(2) . . . . ? 
O1W La1 O17 Mo1 -143.6(3) . . . . ? 
O5W La1 O17 Mo1 -92.3(3) . . . . ? 
O3W La1 O17 Mo1 129.2(3) . . . . ? 
O22 La1 O17 Mo1 -7.4(3) . . . . ? 
O2W La1 O17 Mo1 68.5(3) . . . . ? 
O4W La1 O17 Mo1 169.5(2) . . . . ? 
O14 La1 O17 Mo1 53.0(3) . . . . ? 
O6 La1 O17 Mo1 -62.6(3) . . . . ? 
O6 V1 O18 Mo5 179.99(19) . . . . ? 
O19 V1 O18 Mo5 77.8(2) . . . . ? 
O4 V1 O18 Mo5 -77.9(2) . . . . ? 
O1 V1 O18 Mo5 1.4(6) . . . . ? 
O16 V1 O18 Mo5 0.05(18) . . . . ? 
Mo3 V1 O18 Mo5 -79.6(2) . . . . ? 
O26 Mo5 O18 V1 -179.7(2) . . . . ? 
O20 Mo5 O18 V1 -0.2(6) . . . . ? 
O13 Mo5 O18 V1 78.6(2) . . . . ? 
O8 Mo5 O18 V1 -78.9(2) . . . . ? 
O16 Mo5 O18 V1 -0.05(18) . . . . ? 
Mo4 Mo5 O18 V1 45.31(17) . . . . ? 
Mo6 Mo5 O18 V1 -45.52(17) . . . . ? 
O6 V1 O19 Mo1 70.4(2) . . . . ? 
O18 V1 O19 Mo1 178.17(18) . . . . ? 
O4 V1 O19 Mo1 -62.0(4) . . . . ? 
O1 V1 O19 Mo1 -21.00(16) . . . . ? 
O16 V1 O19 Mo1 -99.82(18) . . . . ? 
Mo3 V1 O19 Mo1 -22.0(2) . . . . ? 
O6 V1 O19 Mo6 -178.40(18) . . . . ? 
O18 V1 O19 Mo6 -70.68(19) . . . . ? 
O4 V1 O19 Mo6 49.1(4) . . . . ? 
O1 V1 O19 Mo6 90.15(17) . . . . ? 
O16 V1 O19 Mo6 11.33(15) . . . . ? 
Mo3 V1 O19 Mo6 89.12(16) . . . . ? 
O23 Mo1 O19 V1 -175.60(19) . . . . ? 
O17 Mo1 O19 V1 -68.5(2) . . . . ? 
O15 Mo1 O19 V1 53.3(4) . . . . ? 
O5 Mo1 O19 V1 95.59(18) . . . . ? 
O1 Mo1 O19 V1 20.28(16) . . . . ? 
Mo2 Mo1 O19 V1 22.5(2) . . . . ? 
O23 Mo1 O19 Mo6 68.82(19) . . . . ? 
O17 Mo1 O19 Mo6 175.93(16) . . . . ? 
O15 Mo1 O19 Mo6 -62.3(3) . . . . ? 
O5 Mo1 O19 Mo6 -20.00(13) . . . . ? 
O1 Mo1 O19 Mo6 -95.31(15) . . . . ? 
Mo2 Mo1 O19 Mo6 -93.05(13) . . . . ? 
O12 Mo6 O19 V1 168.5(2) . . . . ? 
O3 Mo6 O19 V1 -28.3(5) . . . . ? 
O8 Mo6 O19 V1 67.87(18) . . . . ? 
O5 Mo6 O19 V1 -91.96(18) . . . . ? 
O16 Mo6 O19 V1 -11.34(15) . . . . ? 
Mo5 Mo6 O19 V1 34.39(14) . . . . ? 
O12 Mo6 O19 Mo1 -76.78(19) . . . . ? 
O3 Mo6 O19 Mo1 86.4(5) . . . . ? 
O8 Mo6 O19 Mo1 -177.44(18) . . . . ? 
O5 Mo6 O19 Mo1 22.73(15) . . . . ? 
O16 Mo6 O19 Mo1 103.35(17) . . . . ? 
Mo5 Mo6 O19 Mo1 149.08(13) . . . . ? 
O26 Mo5 O20 La2 179.9(3) . . . . ? 
O13 Mo5 O20 La2 -75.7(3) . . . . ? 
O8 Mo5 O20 La2 76.2(3) . . . . ? 
O18 Mo5 O20 La2 0.4(7) . . . . ? 
O16 Mo5 O20 La2 0.2(3) . . . . ? 
Mo4 Mo5 O20 La2 -45.1(3) . . . . ? 
Mo6 Mo5 O20 La2 45.6(3) . . . . ? 
O7W La2 O20 Mo5 -83.5(3) . . . . ? 
O6W La2 O20 Mo5 -179.8(3) . . . . ? 
O9 La2 O20 Mo5 57.9(3) . . . . ? 
O9W La2 O20 Mo5 83.2(4) . . . . ? 
O3 La2 O20 Mo5 -58.5(3) . . . . ? 
O10W La2 O20 Mo5 -137.0(3) . . . . ? 
O8W La2 O20 Mo5 137.8(3) . . . . ? 
O7 La2 O20 Mo5 -0.1(3) . . . . ? 
O25 Mo3 O21 Mo2 -175.8(2) . . . . ? 
O22 Mo3 O21 Mo2 -67.8(2) . . . . ? 
O4 Mo3 O21 Mo2 53.1(4) . . . . ? 
O10 Mo3 O21 Mo2 92.2(2) . . . . ? 
O1 Mo3 O21 Mo2 19.17(18) . . . . ? 
V1 Mo3 O21 Mo2 19.2(2) . . . . ? 
O2 Mo2 O21 Mo3 176.3(2) . . . . ? 
O14 Mo2 O21 Mo3 69.2(2) . . . . ? 
O15 Mo2 O21 Mo3 -43.9(4) . . . . ? 
O11 Mo2 O21 Mo3 -92.6(2) . . . . ? 
O1 Mo2 O21 Mo3 -18.96(18) . . . . ? 
Mo1 Mo2 O21 Mo3 -18.0(2) . . . . ? 
O25 Mo3 O22 La1 176.9(3) . . . . ? 
O21 Mo3 O22 La1 71.6(3) . . . . ? 
O4 Mo3 O22 La1 -81.8(3) . . . . ? 
O10 Mo3 O22 La1 -24.4(6) . . . . ? 
O1 Mo3 O22 La1 -5.7(3) . . . . ? 
V1 Mo3 O22 La1 -48.8(2) . . . . ? 
Mo2 Mo3 O22 La1 41.1(2) . . . . ? 
O1W La1 O22 Mo3 86.6(3) . . . . ? 
O5W La1 O22 Mo3 142.2(3) . . . . ? 
O17 La1 O22 Mo3 6.8(3) . . . . ? 
O3W La1 O22 Mo3 -72.4(3) . . . . ? 
O2W La1 O22 Mo3 -132.7(3) . . . . ? 
O4W La1 O22 Mo3 -170.2(2) . . . . ? 
O14 La1 O22 Mo3 -55.1(3) . . . . ? 
O6 La1 O22 Mo3 62.7(3) . . . . ? 
 
_diffrn_measured_fraction_theta_max    0.998 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.998 
_refine_diff_density_max    0.833 
_refine_diff_density_min   -0.794 
_refine_diff_density_rms    0.156 


#=====================END 
 
data_2
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H36 Ce2 Mo6 O44 V2' 
_chemical_formula_weight          1698.05 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ce'  'Ce'  -0.2486   2.6331 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    10.0173(3) 
_cell_length_b                    10.0913(3) 
_cell_length_c                    19.6748(7) 
_cell_angle_alpha                 77.372(2) 
_cell_angle_beta                  82.719(2) 
_cell_angle_gamma                 78.668(2) 
_cell_volume                      1895.62(10) 
_cell_formula_units_Z             2 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     9084 
_cell_measurement_theta_min       2.08  
_cell_measurement_theta_max       24.99 
 
_exptl_crystal_description        'block' 
_exptl_crystal_colour             'yellow' 
_exptl_crystal_size_max           0.26 
_exptl_crystal_size_mid           0.16 
_exptl_crystal_size_min           0.14 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.975 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              1604 
_exptl_absorpt_coefficient_mu     4.859 
_exptl_absorpt_correction_type    empirical
_exptl_absorpt_correction_T_min   0.409 
_exptl_absorpt_correction_T_max   0.506 
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995'  
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0 
_diffrn_standards_interval_time   0 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             9084 
_diffrn_reflns_av_R_equivalents   0.0189 
_diffrn_reflns_av_sigmaI/netI     0.0426 
_diffrn_reflns_limit_h_min        -11 
_diffrn_reflns_limit_h_max        11 
_diffrn_reflns_limit_k_min        -9 
_diffrn_reflns_limit_k_max        11 
_diffrn_reflns_limit_l_min        -23 
_diffrn_reflns_limit_l_max        23 
_diffrn_reflns_theta_min          2.08 
_diffrn_reflns_theta_max          24.99 
_reflns_number_total              6581 
_reflns_number_gt                 4888 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL'
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0541P)²+5.3846P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.' 
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          6581 
_refine_ls_number_parameters      487 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0549 
_refine_ls_R_factor_gt            0.0373 
_refine_ls_wR_factor_ref          0.1087 
_refine_ls_wR_factor_gt           0.0937 
_refine_ls_goodness_of_fit_ref    1.027 
_refine_ls_restrained_S_all       1.027 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Mo1 Mo 0.50974(7) 0.54596(7) 0.24741(4) 0.01747(17) Uani 1 1 d . . . 
Mo2 Mo 0.22861(7) 0.47857(7) 0.33295(4) 0.02086(18) Uani 1 1 d . . . 
Mo3 Mo 0.22294(7) 0.25465(7) 0.24030(4) 0.01706(17) Uani 1 1 d . . . 
Mo4 Mo 0.48257(7) -0.00418(7) 0.25155(4) 0.01750(17) Uani 1 1 d . . . 
Mo5 Mo 0.76051(7) 0.06441(7) 0.16501(4) 0.02121(18) Uani 1 1 d . . . 
Mo6 Mo 0.76774(7) 0.28753(7) 0.25745(4) 0.01761(17) Uani 1 1 d . . . 
V1 V 0.50316(13) 0.31889(13) 0.15907(7) 0.0133(3) Uani 1 1 d . . . 
V2 V 0.48649(13) 0.22387(13) 0.33945(7) 0.0139(3) Uani 1 1 d . . . 
Ce1 Ce 0.20484(5) 0.63429(5) 0.12850(2) 0.01894(13) Uani 1 1 d . . . 
Ce2 Ce 0.78942(5) -0.09158(5) 0.37039(2) 0.01964(13) Uani 1 1 d . . . 
O1 O 0.5785(6) 0.1023(5) 0.3912(3) 0.0215(13) Uani 1 1 d . . . 
O2 O 0.8347(5) 0.1483(6) 0.3195(3) 0.0218(13) Uani 1 1 d . . . 
O3 O 0.8387(5) 0.2181(5) 0.1751(3) 0.0207(12) Uani 1 1 d . . . 
O4 O 0.4098(5) 0.4400(5) 0.1068(3) 0.0207(12) Uani 1 1 d . . . 
O5 O 0.5820(5) -0.1078(5) 0.3154(3) 0.0222(13) Uani 1 1 d . . . 
O6 O 0.4132(6) 0.6508(6) 0.1829(3) 0.0225(13) Uani 1 1 d . . . 
O7 O 0.1513(6) 0.5940(6) 0.2629(3) 0.0255(14) Uani 1 1 d . . . 
O8 O 0.3824(5) 0.1838(5) 0.1808(3) 0.0169(12) Uani 1 1 d . . . 
O9 O 0.8331(6) -0.0501(6) 0.2347(3) 0.0281(14) Uani 1 1 d . . . 
O10 O 0.3701(5) 0.1167(5) 0.3115(3) 0.0166(12) Uani 1 1 d . . . 
O11 O 0.3862(5) 0.5654(5) 0.3280(3) 0.0207(12) Uani 1 1 d . . . 
O12 O 0.3664(6) 0.3069(5) 0.3922(3) 0.0211(12) Uani 1 1 d . . . 
O13 O 0.6308(6) 0.6357(6) 0.2571(3) 0.0277(14) Uani 1 1 d . . . 
O14 O 0.6037(6) -0.0218(5) 0.1701(3) 0.0228(13) Uani 1 1 d . . . 
O15 O 0.6214(5) 0.2354(5) 0.1064(3) 0.0209(12) Uani 1 1 d . . . 
O16 O 0.8646(6) 0.4105(6) 0.2524(3) 0.0299(15) Uani 1 1 d . . . 
O17 O 0.3630(6) -0.0972(6) 0.2447(3) 0.0248(13) Uani 1 1 d . . . 
O18 O 0.1570(5) 0.3933(5) 0.1768(3) 0.0220(13) Uani 1 1 d . . . 
O19 O 0.8511(6) 0.0232(6) 0.0905(3) 0.0316(15) Uani 1 1 d . . . 
O20 O 0.6047(5) 0.1670(5) 0.2446(3) 0.0171(12) Uani 1 1 d . . . 
O21 O 0.1515(5) 0.3234(5) 0.3228(3) 0.0180(12) Uani 1 1 d . . . 
O22 O 0.1369(6) 0.5195(6) 0.4061(3) 0.0313(15) Uani 1 1 d . . . 
O23 O 0.3867(5) 0.3764(5) 0.2526(3) 0.0175(12) Uani 1 1 d . . . 
O24 O 0.1268(6) 0.1319(6) 0.2441(3) 0.0257(14) Uani 1 1 d . . . 
O25 O 0.6214(5) 0.4268(5) 0.1867(3) 0.0154(11) Uani 1 1 d . . . 
O26 O 0.6089(5) 0.3578(5) 0.3178(3) 0.0173(12) Uani 1 1 d . . . 
O1W O 0.1561(7) 0.5499(7) 0.0254(4) 0.0410(17) Uani 1 1 d . . . 
O2W O 0.3606(6) 0.7497(6) 0.0357(3) 0.0340(15) Uani 1 1 d . . . 
O3W O -0.0499(6) 0.6363(7) 0.1573(4) 0.0379(16) Uani 1 1 d . . . 
O4W O 0.1678(7) 0.8633(6) 0.1664(3) 0.0365(17) Uani 1 1 d . . . 
O5W O 0.0611(6) 0.8260(6) 0.0458(3) 0.0333(15) Uani 1 1 d . . . 
O6W O 0.8418(7) -0.3211(6) 0.3276(4) 0.0423(18) Uani 1 1 d . . . 
O7W O 0.6314(7) -0.2146(9) 0.4615(4) 0.057(2) Uani 1 1 d . . . 
O8W O 0.8586(6) 0.0119(6) 0.4602(3) 0.0334(15) Uani 1 1 d . . . 
O9W O 0.9263(7) -0.2766(6) 0.4540(3) 0.0360(16) Uani 1 1 d . . . 
O10W O 1.0395(6) -0.1074(7) 0.3301(3) 0.0361(16) Uani 1 1 d . . . 
OW1 O -0.0263(7) 0.6949(7) -0.0705(3) 0.0382(16) Uani 1 1 d . . . 
OW2 O -0.0441(7) 0.2573(7) 0.4310(3) 0.0375(16) Uani 1 1 d . . . 
OW3 O 0.5848(7) -0.1401(8) 0.0542(4) 0.0486(19) Uani 1 1 d . . . 
OW4 O 0.2527(7) 0.3991(7) -0.0768(4) 0.0451(18) Uani 1 1 d . . . 
OW5 O 0.2585(8) 1.0934(7) 0.0750(4) 0.0469(19) Uani 1 1 d . . . 
OW6 O 0.4007(8) -0.3096(8) 0.4406(4) 0.051(2) Uani 1 1 d . . . 
OW7 O 0.7723(7) 0.0580(8) 0.5899(4) 0.0465(18) Uani 1 1 d . . . 
OW8 O 0.7040(9) 0.4418(8) 0.4299(4) 0.059(2) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Mo1 O13 1.701(6) . ? 
Mo1 O6 1.729(5) . ? 
Mo1 O11 1.905(6) . ? 
Mo1 O25 1.971(5) . ? 
Mo1 O26 2.229(5) . ? 
Mo1 O23 2.276(5) . ? 
Mo1 Mo2 3.2058(10) . ? 
Mo2 O22 1.691(6) . ? 
Mo2 O7 1.752(5) . ? 
Mo2 O21 1.934(5) . ? 
Mo2 O11 1.933(5) . ? 
Mo2 O12 2.202(5) . ? 
Mo2 O23 2.347(5) . ? 
Mo2 Mo3 3.2109(10) . ? 
Mo3 O24 1.696(5) . ? 
Mo3 O18 1.742(5) . ? 
Mo3 O21 1.905(5) . ? 
Mo3 O8 1.969(5) . ? 
Mo3 O10 2.222(5) . ? 
Mo3 O23 2.297(5) . ? 
Mo3 V1 3.1590(14) . ? 
Mo4 O17 1.694(5) . ? 
Mo4 O5 1.731(5) . ? 
Mo4 O14 1.902(6) . ? 
Mo4 O10 1.975(5) . ? 
Mo4 O8 2.234(5) . ? 
Mo4 O20 2.277(5) . ? 
Mo4 Mo5 3.1891(10) . ? 
Mo5 O19 1.711(6) . ? 
Mo5 O9 1.724(6) . ? 
Mo5 O3 1.925(5) . ? 
Mo5 O14 1.922(6) . ? 
Mo5 O15 2.200(5) . ? 
Mo5 O20 2.326(5) . ? 
Mo5 Mo6 3.2046(10) . ? 
Mo6 O16 1.699(6) . ? 
Mo6 O2 1.733(5) . ? 
Mo6 O3 1.906(5) . ? 
Mo6 O26 1.973(5) . ? 
Mo6 O25 2.217(5) . ? 
Mo6 O20 2.287(5) . ? 
V1 O4 1.634(5) . ? 
V1 O15 1.693(5) . ? 
V1 O25 1.952(5) . ? 
V1 O8 1.940(5) . ? 
V1 O23 2.177(5) . ? 
V1 O20 2.216(5) . ? 
V2 O1 1.625(5) . ? 
V2 O12 1.702(6) . ? 
V2 O10 1.936(5) . ? 
V2 O26 1.944(5) . ? 
V2 O20 2.204(5) . ? 
V2 O23 2.229(5) . ? 
Ce1 O2W 2.486(6) . ? 
Ce1 O6 2.512(5) . ? 
Ce1 O18 2.526(5) . ? 
Ce1 O1W 2.500(6) . ? 
Ce1 O4W 2.526(6) . ? 
Ce1 O3W 2.539(6) . ? 
Ce1 O5W 2.566(6) . ? 
Ce1 O7 2.588(6) . ? 
Ce1 O4 2.608(5) . ? 
Ce2 O8W 2.469(6) . ? 
Ce2 O2 2.515(5) . ? 
Ce2 O9W 2.509(6) . ? 
Ce2 O5 2.509(5) . ? 
Ce2 O7W 2.517(7) . ? 
Ce2 O10W 2.514(6) . ? 
Ce2 O9 2.604(6) . ? 
Ce2 O6W 2.571(6) . ? 
Ce2 O1 2.639(5) . ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O13 Mo1 O6 105.8(3) . . ? 
O13 Mo1 O11 101.7(3) . . ? 
O6 Mo1 O11 100.2(2) . . ? 
O13 Mo1 O25 98.4(2) . . ? 
O6 Mo1 O25 95.9(2) . . ? 
O11 Mo1 O25 149.5(2) . . ? 
O13 Mo1 O26 91.4(2) . . ? 
O6 Mo1 O26 161.0(2) . . ? 
O11 Mo1 O26 83.5(2) . . ? 
O25 Mo1 O26 73.3(2) . . ? 
O13 Mo1 O23 163.8(2) . . ? 
O6 Mo1 O23 89.9(2) . . ? 
O11 Mo1 O23 78.5(2) . . ? 
O25 Mo1 O23 75.9(2) . . ? 
O26 Mo1 O23 72.49(18) . . ? 
O13 Mo1 Mo2 135.3(2) . . ? 
O6 Mo1 Mo2 87.54(19) . . ? 
O11 Mo1 Mo2 33.63(16) . . ? 
O25 Mo1 Mo2 122.83(15) . . ? 
O26 Mo1 Mo2 85.54(14) . . ? 
O23 Mo1 Mo2 47.01(13) . . ? 
O22 Mo2 O7 105.7(3) . . ? 
O22 Mo2 O21 101.2(3) . . ? 
O7 Mo2 O21 95.3(2) . . ? 
O22 Mo2 O11 102.2(3) . . ? 
O7 Mo2 O11 96.7(3) . . ? 
O21 Mo2 O11 149.7(2) . . ? 
O22 Mo2 O12 93.1(2) . . ? 
O7 Mo2 O12 161.1(2) . . ? 
O21 Mo2 O12 79.5(2) . . ? 
O11 Mo2 O12 80.2(2) . . ? 
O22 Mo2 O23 165.1(2) . . ? 
O7 Mo2 O23 89.2(2) . . ? 
O21 Mo2 O23 76.2(2) . . ? 
O11 Mo2 O23 76.2(2) . . ? 
O12 Mo2 O23 71.94(19) . . ? 
O22 Mo2 Mo1 135.2(2) . . ? 
O7 Mo2 Mo1 84.76(19) . . ? 
O21 Mo2 Mo1 121.44(15) . . ? 
O11 Mo2 Mo1 33.09(16) . . ? 
O12 Mo2 Mo1 82.64(15) . . ? 
O23 Mo2 Mo1 45.20(13) . . ? 
O22 Mo2 Mo3 134.0(2) . . ? 
O7 Mo2 Mo3 83.25(19) . . ? 
O21 Mo2 Mo3 32.96(15) . . ? 
O11 Mo2 Mo3 121.78(16) . . ? 
O12 Mo2 Mo3 82.67(14) . . ? 
O23 Mo2 Mo3 45.63(13) . . ? 
Mo1 Mo2 Mo3 89.80(2) . . ? 
O24 Mo3 O18 105.4(3) . . ? 
O24 Mo3 O21 101.4(3) . . ? 
O18 Mo3 O21 100.2(2) . . ? 
O24 Mo3 O8 99.1(2) . . ? 
O18 Mo3 O8 96.4(2) . . ? 
O21 Mo3 O8 149.0(2) . . ? 
O24 Mo3 O10 93.7(2) . . ? 
O18 Mo3 O10 159.5(2) . . ? 
O21 Mo3 O10 82.6(2) . . ? 
O8 Mo3 O10 73.1(2) . . ? 
O24 Mo3 O23 165.5(2) . . ? 
O18 Mo3 O23 88.8(2) . . ? 
O21 Mo3 O23 78.0(2) . . ? 
O8 Mo3 O23 76.33(19) . . ? 
O10 Mo3 O23 71.81(18) . . ? 
O24 Mo3 V1 134.6(2) . . ? 
O18 Mo3 V1 82.06(18) . . ? 
O21 Mo3 V1 121.59(16) . . ? 
O8 Mo3 V1 35.79(14) . . ? 
O10 Mo3 V1 79.30(14) . . ? 
O23 Mo3 V1 43.56(13) . . ? 
O24 Mo3 Mo2 134.8(2) . . ? 
O18 Mo3 Mo2 86.42(19) . . ? 
O21 Mo3 Mo2 33.54(16) . . ? 
O8 Mo3 Mo2 123.16(14) . . ? 
O10 Mo3 Mo2 85.03(13) . . ? 
O23 Mo3 Mo2 46.90(13) . . ? 
V1 Mo3 Mo2 89.60(3) . . ? 
O17 Mo4 O5 104.8(3) . . ? 
O17 Mo4 O14 102.5(3) . . ? 
O5 Mo4 O14 100.4(3) . . ? 
O17 Mo4 O10 98.1(2) . . ? 
O5 Mo4 O10 96.9(2) . . ? 
O14 Mo4 O10 148.6(2) . . ? 
O17 Mo4 O8 93.0(2) . . ? 
O5 Mo4 O8 160.6(2) . . ? 
O14 Mo4 O8 82.7(2) . . ? 
O10 Mo4 O8 72.7(2) . . ? 
O17 Mo4 O20 164.8(2) . . ? 
O5 Mo4 O20 89.8(2) . . ? 
O14 Mo4 O20 78.0(2) . . ? 
O10 Mo4 O20 75.98(19) . . ? 
O8 Mo4 O20 71.97(18) . . ? 
O17 Mo4 Mo5 136.1(2) . . ? 
O5 Mo4 Mo5 87.08(19) . . ? 
O14 Mo4 Mo5 33.69(16) . . ? 
O10 Mo4 Mo5 122.69(15) . . ? 
O8 Mo4 Mo5 85.17(14) . . ? 
O20 Mo4 Mo5 46.79(13) . . ? 
O19 Mo5 O9 107.1(3) . . ? 
O19 Mo5 O3 101.4(3) . . ? 
O9 Mo5 O3 95.9(3) . . ? 
O19 Mo5 O14 101.7(3) . . ? 
O9 Mo5 O14 95.5(3) . . ? 
O3 Mo5 O14 150.0(2) . . ? 
O19 Mo5 O15 92.9(2) . . ? 
O9 Mo5 O15 160.0(2) . . ? 
O3 Mo5 O15 80.0(2) . . ? 
O14 Mo5 O15 79.8(2) . . ? 
O19 Mo5 O20 164.4(2) . . ? 
O9 Mo5 O20 88.5(2) . . ? 
O3 Mo5 O20 76.2(2) . . ? 
O14 Mo5 O20 76.4(2) . . ? 
O15 Mo5 O20 71.50(19) . . ? 
O19 Mo5 Mo4 134.9(2) . . ? 
O9 Mo5 Mo4 82.9(2) . . ? 
O3 Mo5 Mo4 121.68(16) . . ? 
O14 Mo5 Mo4 33.30(16) . . ? 
O15 Mo5 Mo4 82.71(14) . . ? 
O20 Mo5 Mo4 45.51(13) . . ? 
O19 Mo5 Mo6 134.3(2) . . ? 
O9 Mo5 Mo6 83.3(2) . . ? 
O3 Mo5 Mo6 33.04(16) . . ? 
O14 Mo5 Mo6 121.90(16) . . ? 
O15 Mo5 Mo6 82.81(14) . . ? 
O20 Mo5 Mo6 45.50(13) . . ? 
Mo4 Mo5 Mo6 89.82(2) . . ? 
O16 Mo6 O2 106.0(3) . . ? 
O16 Mo6 O3 100.9(3) . . ? 
O2 Mo6 O3 99.1(2) . . ? 
O16 Mo6 O26 99.6(3) . . ? 
O2 Mo6 O26 96.7(2) . . ? 
O3 Mo6 O26 149.4(2) . . ? 
O16 Mo6 O25 92.9(2) . . ? 
O2 Mo6 O25 160.0(2) . . ? 
O3 Mo6 O25 82.9(2) . . ? 
O26 Mo6 O25 73.5(2) . . ? 
O16 Mo6 O20 165.0(2) . . ? 
O2 Mo6 O20 88.9(2) . . ? 
O3 Mo6 O20 77.5(2) . . ? 
O26 Mo6 O20 76.72(19) . . ? 
O25 Mo6 O20 72.03(18) . . ? 
O16 Mo6 Mo5 134.3(2) . . ? 
O2 Mo6 Mo5 85.79(19) . . ? 
O3 Mo6 Mo5 33.43(16) . . ? 
O26 Mo6 Mo5 123.18(15) . . ? 
O25 Mo6 Mo5 85.31(13) . . ? 
O20 Mo6 Mo5 46.51(13) . . ? 
O4 V1 O15 105.8(3) . . ? 
O4 V1 O25 100.3(2) . . ? 
O15 V1 O25 97.7(2) . . ? 
O4 V1 O8 98.8(2) . . ? 
O15 V1 O8 96.9(2) . . ? 
O25 V1 O8 151.8(2) . . ? 
O4 V1 O23 92.9(2) . . ? 
O15 V1 O23 161.3(2) . . ? 
O25 V1 O23 78.6(2) . . ? 
O8 V1 O23 79.9(2) . . ? 
O4 V1 O20 170.1(2) . . ? 
O15 V1 O20 84.1(2) . . ? 
O25 V1 O20 78.7(2) . . ? 
O8 V1 O20 79.0(2) . . ? 
O23 V1 O20 77.17(19) . . ? 
O4 V1 Mo3 85.72(19) . . ? 
O15 V1 Mo3 133.20(19) . . ? 
O25 V1 Mo3 125.30(16) . . ? 
O8 V1 Mo3 36.39(16) . . ? 
O23 V1 Mo3 46.66(14) . . ? 
O20 V1 Mo3 86.92(14) . . ? 
O1 V2 O12 106.0(3) . . ? 
O1 V2 O10 99.7(3) . . ? 
O12 V2 O10 97.5(2) . . ? 
O1 V2 O26 98.9(3) . . ? 
O12 V2 O26 97.8(2) . . ? 
O10 V2 O26 151.6(2) . . ? 
O1 V2 O20 93.0(2) . . ? 
O12 V2 O20 161.0(2) . . ? 
O10 V2 O20 78.5(2) . . ? 
O26 V2 O20 79.3(2) . . ? 
O1 V2 O23 169.3(3) . . ? 
O12 V2 O23 84.6(2) . . ? 
O10 V2 O23 78.7(2) . . ? 
O26 V2 O23 79.0(2) . . ? 
O20 V2 O23 76.35(19) . . ? 
O2W Ce1 O6 71.72(19) . . ? 
O2W Ce1 O18 137.9(2) . . ? 
O6 Ce1 O18 105.99(17) . . ? 
O2W Ce1 O1W 79.7(2) . . ? 
O6 Ce1 O1W 136.7(2) . . ? 
O18 Ce1 O1W 74.8(2) . . ? 
O2W Ce1 O4W 82.0(2) . . ? 
O6 Ce1 O4W 71.08(19) . . ? 
O18 Ce1 O4W 138.5(2) . . ? 
O1W Ce1 O4W 136.4(2) . . ? 
O2W Ce1 O3W 138.5(2) . . ? 
O6 Ce1 O3W 141.1(2) . . ? 
O18 Ce1 O3W 69.10(18) . . ? 
O1W Ce1 O3W 80.8(2) . . ? 
O4W Ce1 O3W 87.5(2) . . ? 
O2W Ce1 O5W 71.1(2) . . ? 
O6 Ce1 O5W 127.34(19) . . ? 
O18 Ce1 O5W 126.59(19) . . ? 
O1W Ce1 O5W 68.7(2) . . ? 
O4W Ce1 O5W 68.0(2) . . ? 
O3W Ce1 O5W 67.7(2) . . ? 
O2W Ce1 O7 139.58(19) . . ? 
O6 Ce1 O7 71.27(18) . . ? 
O18 Ce1 O7 69.04(18) . . ? 
O1W Ce1 O7 140.1(2) . . ? 
O4W Ce1 O7 71.2(2) . . ? 
O3W Ce1 O7 71.1(2) . . ? 
O5W Ce1 O7 121.94(19) . . ? 
O2W Ce1 O4 74.98(19) . . ? 
O6 Ce1 O4 67.99(17) . . ? 
O18 Ce1 O4 66.03(17) . . ? 
O1W Ce1 O4 73.75(19) . . ? 
O4W Ce1 O4 137.51(19) . . ? 
O3W Ce1 O4 132.66(19) . . ? 
O5W Ce1 O4 132.81(19) . . ? 
O7 Ce1 O4 105.17(17) . . ? 
O8W Ce2 O2 69.08(19) . . ? 
O8W Ce2 O9W 70.8(2) . . ? 
O2 Ce2 O9W 127.70(19) . . ? 
O8W Ce2 O5 141.40(19) . . ? 
O2 Ce2 O5 104.64(17) . . ? 
O9W Ce2 O5 127.63(19) . . ? 
O8W Ce2 O7W 89.9(2) . . ? 
O2 Ce2 O7W 140.1(2) . . ? 
O9W Ce2 O7W 70.1(2) . . ? 
O5 Ce2 O7W 70.7(2) . . ? 
O8W Ce2 O10W 81.6(2) . . ? 
O2 Ce2 O10W 71.82(19) . . ? 
O9W Ce2 O10W 70.4(2) . . ? 
O5 Ce2 O10W 134.3(2) . . ? 
O7W Ce2 O10W 140.3(2) . . ? 
O8W Ce2 O9 133.4(2) . . ? 
O2 Ce2 O9 68.37(18) . . ? 
O9W Ce2 O9 125.06(19) . . ? 
O5 Ce2 O9 68.77(18) . . ? 
O7W Ce2 O9 135.9(2) . . ? 
O10W Ce2 O9 67.9(2) . . ? 
O8W Ce2 O6W 139.0(2) . . ? 
O2 Ce2 O6W 134.6(2) . . ? 
O9W Ce2 O6W 69.0(2) . . ? 
O5 Ce2 O6W 73.29(18) . . ? 
O7W Ce2 O6W 83.5(3) . . ? 
O10W Ce2 O6W 78.4(2) . . ? 
O9 Ce2 O6W 69.0(2) . . ? 
O8W Ce2 O1 76.26(18) . . ? 
O2 Ce2 O1 66.78(17) . . ? 
O9W Ce2 O1 131.72(19) . . ? 
O5 Ce2 O1 66.87(17) . . ? 
O7W Ce2 O1 75.6(2) . . ? 
O10W Ce2 O1 137.73(19) . . ? 
O9 Ce2 O1 103.22(17) . . ? 
O6W Ce2 O1 139.19(19) . . ? 
V2 O1 Ce2 133.8(3) . . ? 
Mo6 O2 Ce2 137.0(3) . . ? 
Mo5 O3 Mo6 113.5(3) . . ? 
V1 O4 Ce1 133.1(3) . . ? 
Mo4 O5 Ce2 136.1(3) . . ? 
Mo1 O6 Ce1 134.9(3) . . ? 
Mo2 O7 Ce1 133.7(3) . . ? 
V1 O8 Mo3 107.8(2) . . ? 
V1 O8 Mo4 108.8(2) . . ? 
Mo3 O8 Mo4 103.1(2) . . ? 
Mo5 O9 Ce2 136.1(3) . . ? 
V2 O10 Mo4 108.6(2) . . ? 
V2 O10 Mo3 109.7(2) . . ? 
Mo4 O10 Mo3 103.3(2) . . ? 
Mo1 O11 Mo2 113.3(3) . . ? 
V2 O12 Mo2 112.6(3) . . ? 
Mo5 O14 Mo4 113.0(3) . . ? 
V1 O15 Mo5 112.9(3) . . ? 
Mo3 O18 Ce1 135.5(3) . . ? 
V2 O20 V1 103.0(2) . . ? 
V2 O20 Mo4 90.23(19) . . ? 
V1 O20 Mo4 98.34(19) . . ? 
V2 O20 Mo6 89.83(18) . . ? 
V1 O20 Mo6 98.1(2) . . ? 
Mo4 O20 Mo6 163.1(3) . . ? 
V2 O20 Mo5 165.4(3) . . ? 
V1 O20 Mo5 91.54(19) . . ? 
Mo4 O20 Mo5 87.70(17) . . ? 
Mo6 O20 Mo5 88.00(18) . . ? 
Mo3 O21 Mo2 113.5(3) . . ? 
V1 O23 V2 103.5(2) . . ? 
V1 O23 Mo1 91.1(2) . . ? 
V2 O23 Mo1 97.74(19) . . ? 
V1 O23 Mo3 89.78(19) . . ? 
V2 O23 Mo3 97.5(2) . . ? 
Mo1 O23 Mo3 164.1(2) . . ? 
V1 O23 Mo2 165.7(3) . . ? 
V2 O23 Mo2 90.83(19) . . ? 
Mo1 O23 Mo2 87.79(18) . . ? 
Mo3 O23 Mo2 87.47(18) . . ? 
V1 O25 Mo1 108.2(2) . . ? 
V1 O25 Mo6 109.2(2) . . ? 
Mo1 O25 Mo6 103.0(2) . . ? 
V2 O26 Mo6 108.1(2) . . ? 
V2 O26 Mo1 108.6(2) . . ? 
Mo6 O26 Mo1 102.6(2) . . ? 
 
_diffrn_measured_fraction_theta_max    0.988 
_diffrn_reflns_theta_full              24.99 
_diffrn_measured_fraction_theta_full   0.988 
_refine_diff_density_max    1.134 
_refine_diff_density_min   -0.980 
_refine_diff_density_rms    0.198 


#=====================END 

 
data_3 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'H36 Mo6 Nd2 O44 V2' 
_chemical_formula_weight          1706.29 
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'V'  'V'   0.3005   0.5294 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Mo'  'Mo'  -1.6832   0.6857 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Nd'  'Nd'  -0.1943   3.0179 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            Triclinic  
_symmetry_space_group_name_H-M    P-1  
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    10.038(5) 
_cell_length_b                    10.049(6) 
_cell_length_c                    10.118(6) 
_cell_angle_alpha                 106.967(8) 
_cell_angle_beta                  101.480(9) 
_cell_angle_gamma                 91.502(8) 
_cell_volume                      952.8(9) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     4586
_cell_measurement_theta_min       2.08
_cell_measurement_theta_max       25.00  
 
_exptl_crystal_description        'block' 
_exptl_crystal_colour             'yellow' 
_exptl_crystal_size_max           0.19 
_exptl_crystal_size_mid           0.15 
_exptl_crystal_size_min           0.14 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     2.974 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              806 
_exptl_absorpt_coefficient_mu     5.169 
_exptl_absorpt_correction_type    empirical 
_exptl_absorpt_correction_T_min   0.410
_exptl_absorpt_correction_T_max   0.485  
_exptl_absorpt_process_details    'ABSCOR by T.Higashi 8 March, 1995'
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker Smart Apex CCD' 
_diffrn_measurement_method        'ω-2θ' 
_diffrn_detector_area_resol_mean  0.01 
_diffrn_standards_number          0 
_diffrn_standards_interval_count  0  
_diffrn_standards_interval_time   0  
_diffrn_standards_decay_%         none  
_diffrn_reflns_number             4586 
_diffrn_reflns_av_R_equivalents   0.0412 
_diffrn_reflns_av_sigmaI/netI     0.0898 
_diffrn_reflns_limit_h_min        -6 
_diffrn_reflns_limit_h_max        11 
_diffrn_reflns_limit_k_min        -11 
_diffrn_reflns_limit_k_max        11 
_diffrn_reflns_limit_l_min        -12 
_diffrn_reflns_limit_l_max        11 
_diffrn_reflns_theta_min          2.08 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              3293 
_reflns_number_gt                 2140 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        ? 
_computing_cell_refinement        ? 
_computing_data_reduction         ? 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL'
_computing_publication_material   'Bruker SHELXTL' 
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0800P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    '.'
_refine_ls_hydrogen_treatment     none 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          3293 
_refine_ls_number_parameters      244 
_refine_ls_number_restraints      0 
_refine_ls_R_factor_all           0.0917 
_refine_ls_R_factor_gt            0.0568 
_refine_ls_wR_factor_ref          0.1661 
_refine_ls_wR_factor_gt           0.1454 
_refine_ls_goodness_of_fit_ref    1.028 
_refine_ls_restrained_S_all       1.028 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
 
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Nd1 Nd 0.29227(8) 0.25810(8) 0.24197(11) 0.0402(3) Uani 1 1 d . . . 
Mo1 Mo 0.26562(12) 0.66790(12) 0.29133(16) 0.0372(4) Uani 1 1 d . . . 
Mo2 Mo 0.27216(11) 0.48318(12) -0.02453(15) 0.0315(4) Uani 1 1 d . . . 
Mo3 Mo -0.01377(11) 0.49610(12) 0.27284(15) 0.0309(4) Uani 1 1 d . . . 
V1 V 0.0086(2) 0.6795(2) 0.0430(3) 0.0274(6) Uani 1 1 d . . . 
O1 O 0.3379(8) 0.3590(9) 0.0507(11) 0.032(2) Uani 1 1 d . . . 
O2 O 0.1081(9) 0.6567(10) 0.3709(11) 0.036(3) Uani 1 1 d . . . 
O3 O 0.0830(9) 0.3693(9) 0.3123(11) 0.034(2) Uani 1 1 d . . . 
O4 O 0.3427(8) 0.6475(9) 0.1267(11) 0.033(2) Uani 1 1 d . . . 
O5 O -0.1245(8) 0.3745(8) 0.0926(11) 0.030(2) Uani 1 1 d . . . 
O6 O 0.3571(10) 0.8149(10) 0.4058(13) 0.048(3) Uani 1 1 d . . . 
O7 O 0.3678(9) 0.4942(10) -0.1402(12) 0.042(3) Uani 1 1 d . . . 
O8 O -0.1334(9) 0.5146(10) 0.3718(12) 0.045(3) Uani 1 1 d . . . 
O9 O 0.1278(8) 0.7851(9) 0.1798(11) 0.034(3) Uani 1 1 d . . . 
O10 O 0.0829(9) 0.2161(9) 0.0268(11) 0.034(2) Uani 1 1 d . . . 
O11 O 0.1083(8) 0.5084(8) 0.1086(11) 0.031(2) Uani 1 1 d . . . 
O12 O 0.3399(9) 0.5309(10) 0.3359(12) 0.040(3) Uani 1 1 d . . . 
O13 O 0.1135(8) 0.3640(8) -0.1558(10) 0.025(2) Uani 1 1 d . . . 
O1W O 0.3527(11) 0.0652(13) 0.0478(16) 0.083(5) Uani 1 1 d . . . 
O2W O 0.4360(11) 0.0898(11) 0.3485(13) 0.051(3) Uani 1 1 d . . . 
O3W O 0.1362(10) 0.0728(11) 0.2738(14) 0.055(3) Uani 1 1 d . . . 
O4W O 0.3387(11) 0.3408(12) 0.5154(12) 0.054(3) Uani 1 1 d . . . 
O5W O 0.5478(9) 0.3272(12) 0.2896(12) 0.048(3) Uani 1 1 d . . . 
OW1 O 0.2224(15) 0.1471(13) -0.3504(17) 0.081(4) Uani 1 1 d . . . 
OW2 O 0.0909(13) 0.8871(13) 0.6053(17) 0.079(5) Uani 1 1 d . . . 
OW3 O -0.2569(13) 0.1663(13) 0.1668(14) 0.067(4) Uani 1 1 d . . . 
OW4 O 0.5343(11) 0.8601(11) 0.1575(17) 0.070(4) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Nd1 O1W 2.510(12) . ? 
Nd1 O3W 2.535(10) . ? 
Nd1 O3 2.534(9) . ? 
Nd1 O1 2.541(10) . ? 
Nd1 O5W 2.552(9) . ? 
Nd1 O2W 2.584(10) . ? 
Nd1 O4W 2.586(12) . ? 
Nd1 O12 2.622(10) . ? 
Nd1 O10 2.632(10) . ? 
Mo1 O6 1.695(10) . ? 
Mo1 O12 1.714(10) . ? 
Mo1 O2 1.926(9) . ? 
Mo1 O4 1.933(10) . ? 
Mo1 O9 2.194(9) . ? 
Mo1 O11 2.336(9) . ? 
Mo1 Mo3 3.198(2) . ? 
Mo1 Mo2 3.208(3) . ? 
Mo2 O7 1.680(10) . ? 
Mo2 O1 1.723(9) . ? 
Mo2 O4 1.898(9) . ? 
Mo2 O13 1.965(9) . ? 
Mo2 O5 2.236(9) 2_565 ? 
Mo2 O11 2.300(9) . ? 
Mo2 V1 3.165(3) 2_565 ? 
Mo3 O8 1.691(9) . ? 
Mo3 O3 1.713(9) . ? 
Mo3 O2 1.887(9) . ? 
Mo3 O5 1.969(10) . ? 
Mo3 O13 2.226(9) 2_565 ? 
Mo3 O11 2.280(10) . ? 
V1 O10 1.634(10) 2_565 ? 
V1 O9 1.700(9) . ? 
V1 O5 1.940(9) 2_565 ? 
V1 O13 1.953(9) 2_565 ? 
V1 O11 2.184(9) 2_565 ? 
V1 O11 2.211(9) . ? 
V1 Mo2 3.165(3) 2_565 ? 
O5 V1 1.940(9) 2_565 ? 
O5 Mo2 2.236(9) 2_565 ? 
O10 V1 1.634(10) 2_565 ? 
O11 V1 2.184(9) 2_565 ? 
O13 V1 1.953(9) 2_565 ? 
O13 Mo3 2.226(9) 2_565 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1W Nd1 O3W 86.0(4) . . ? 
O1W Nd1 O3 139.4(3) . . ? 
O3W Nd1 O3 71.7(3) . . ? 
O1W Nd1 O1 71.5(4) . . ? 
O3W Nd1 O1 140.2(4) . . ? 
O3 Nd1 O1 104.5(3) . . ? 
O1W Nd1 O5W 81.0(4) . . ? 
O3W Nd1 O5W 138.2(4) . . ? 
O3 Nd1 O5W 137.5(3) . . ? 
O1 Nd1 O5W 71.4(3) . . ? 
O1W Nd1 O2W 70.1(4) . . ? 
O3W Nd1 O2W 70.1(3) . . ? 
O3 Nd1 O2W 128.1(4) . . ? 
O1 Nd1 O2W 127.3(3) . . ? 
O5W Nd1 O2W 68.1(4) . . ? 
O1W Nd1 O4W 138.5(4) . . ? 
O3W Nd1 O4W 81.9(4) . . ? 
O3 Nd1 O4W 72.5(3) . . ? 
O1 Nd1 O4W 136.2(4) . . ? 
O5W Nd1 O4W 82.1(4) . . ? 
O2W Nd1 O4W 68.5(4) . . ? 
O1W Nd1 O12 135.9(4) . . ? 
O3W Nd1 O12 137.3(3) . . ? 
O3 Nd1 O12 69.5(3) . . ? 
O1 Nd1 O12 68.2(3) . . ? 
O5W Nd1 O12 70.0(3) . . ? 
O2W Nd1 O12 123.8(3) . . ? 
O4W Nd1 O12 70.2(4) . . ? 
O1W Nd1 O10 75.2(3) . . ? 
O3W Nd1 O10 76.4(4) . . ? 
O3 Nd1 O10 66.9(3) . . ? 
O1 Nd1 O10 66.4(3) . . ? 
O5W Nd1 O10 136.2(3) . . ? 
O2W Nd1 O10 132.6(3) . . ? 
O4W Nd1 O10 138.2(3) . . ? 
O12 Nd1 O10 103.5(3) . . ? 
O6 Mo1 O12 106.1(5) . . ? 
O6 Mo1 O2 102.6(5) . . ? 
O12 Mo1 O2 96.2(4) . . ? 
O6 Mo1 O4 101.1(5) . . ? 
O12 Mo1 O4 95.6(5) . . ? 
O2 Mo1 O4 149.3(4) . . ? 
O6 Mo1 O9 93.0(4) . . ? 
O12 Mo1 O9 160.8(4) . . ? 
O2 Mo1 O9 79.9(4) . . ? 
O4 Mo1 O9 79.7(4) . . ? 
O6 Mo1 O11 164.6(4) . . ? 
O12 Mo1 O11 89.3(4) . . ? 
O2 Mo1 O11 75.8(4) . . ? 
O4 Mo1 O11 76.1(4) . . ? 
O9 Mo1 O11 71.6(3) . . ? 
O6 Mo1 Mo3 135.2(4) . . ? 
O12 Mo1 Mo3 84.1(3) . . ? 
O2 Mo1 Mo3 32.6(3) . . ? 
O4 Mo1 Mo3 121.6(3) . . ? 
O9 Mo1 Mo3 82.7(2) . . ? 
O11 Mo1 Mo3 45.4(2) . . ? 
O6 Mo1 Mo2 133.8(4) . . ? 
O12 Mo1 Mo2 83.4(4) . . ? 
O2 Mo1 Mo2 121.5(3) . . ? 
O4 Mo1 Mo2 32.8(3) . . ? 
O9 Mo1 Mo2 82.8(3) . . ? 
O11 Mo1 Mo2 45.8(2) . . ? 
Mo3 Mo1 Mo2 90.04(5) . . ? 
O7 Mo2 O1 106.2(5) . . ? 
O7 Mo2 O4 100.6(4) . . ? 
O1 Mo2 O4 99.7(4) . . ? 
O7 Mo2 O13 99.7(4) . . ? 
O1 Mo2 O13 96.8(4) . . ? 
O4 Mo2 O13 149.0(3) . . ? 
O7 Mo2 O5 93.0(4) . 2_565 ? 
O1 Mo2 O5 159.8(4) . 2_565 ? 
O4 Mo2 O5 82.7(4) . 2_565 ? 
O13 Mo2 O5 73.1(3) . 2_565 ? 
O7 Mo2 O11 164.8(4) . . ? 
O1 Mo2 O11 89.0(4) . . ? 
O4 Mo2 O11 77.7(3) . . ? 
O13 Mo2 O11 76.6(3) . . ? 
O5 Mo2 O11 71.8(3) 2_565 . ? 
O7 Mo2 V1 135.5(4) . 2_565 ? 
O1 Mo2 V1 82.4(3) . 2_565 ? 
O4 Mo2 V1 121.3(3) . 2_565 ? 
O13 Mo2 V1 36.0(3) . 2_565 ? 
O5 Mo2 V1 79.3(2) 2_565 2_565 ? 
O11 Mo2 V1 43.6(2) . 2_565 ? 
O7 Mo2 Mo1 134.0(3) . . ? 
O1 Mo2 Mo1 86.1(3) . . ? 
O4 Mo2 Mo1 33.5(3) . . ? 
O13 Mo2 Mo1 123.2(3) . . ? 
O5 Mo2 Mo1 85.2(3) 2_565 . ? 
O11 Mo2 Mo1 46.7(2) . . ? 
V1 Mo2 Mo1 89.41(6) 2_565 . ? 
O8 Mo3 O3 106.0(5) . . ? 
O8 Mo3 O2 102.0(5) . . ? 
O3 Mo3 O2 100.3(4) . . ? 
O8 Mo3 O5 98.8(4) . . ? 
O3 Mo3 O5 96.0(4) . . ? 
O2 Mo3 O5 148.8(4) . . ? 
O8 Mo3 O13 91.6(4) . 2_565 ? 
O3 Mo3 O13 160.8(4) . 2_565 ? 
O2 Mo3 O13 83.1(4) . 2_565 ? 
O5 Mo3 O13 73.2(3) . 2_565 ? 
O8 Mo3 O11 163.7(4) . . ? 
O3 Mo3 O11 90.0(4) . . ? 
O2 Mo3 O11 77.9(4) . . ? 
O5 Mo3 O11 75.7(3) . . ? 
O13 Mo3 O11 72.1(3) 2_565 . ? 
O8 Mo3 Mo1 135.3(4) . . ? 
O3 Mo3 Mo1 87.3(3) . . ? 
O2 Mo3 Mo1 33.4(3) . . ? 
O5 Mo3 Mo1 122.5(3) . . ? 
O13 Mo3 Mo1 85.5(2) 2_565 . ? 
O11 Mo3 Mo1 46.9(2) . . ? 
O10 V1 O9 105.8(5) 2_565 . ? 
O10 V1 O5 98.9(5) 2_565 2_565 ? 
O9 V1 O5 97.8(4) . 2_565 ? 
O10 V1 O13 99.3(4) 2_565 2_565 ? 
O9 V1 O13 97.1(5) . 2_565 ? 
O5 V1 O13 152.2(4) 2_565 2_565 ? 
O10 V1 O11 93.2(4) 2_565 2_565 ? 
O9 V1 O11 161.0(4) . 2_565 ? 
O5 V1 O11 78.6(4) 2_565 2_565 ? 
O13 V1 O11 79.7(4) 2_565 2_565 ? 
O10 V1 O11 169.9(4) 2_565 . ? 
O9 V1 O11 84.3(4) . . ? 
O5 V1 O11 79.4(4) 2_565 . ? 
O13 V1 O11 78.9(3) 2_565 . ? 
O11 V1 O11 76.8(4) 2_565 . ? 
O10 V1 Mo2 86.3(3) 2_565 2_565 ? 
O9 V1 Mo2 133.4(4) . 2_565 ? 
O5 V1 Mo2 125.2(3) 2_565 2_565 ? 
O13 V1 Mo2 36.3(3) 2_565 2_565 ? 
O11 V1 Mo2 46.6(2) 2_565 2_565 ? 
O11 V1 Mo2 86.6(2) . 2_565 ? 
Mo2 O1 Nd1 136.6(5) . . ? 
Mo3 O2 Mo1 114.0(5) . . ? 
Mo3 O3 Nd1 135.9(5) . . ? 
Mo2 O4 Mo1 113.7(4) . . ? 
V1 O5 Mo3 108.8(4) 2_565 . ? 
V1 O5 Mo2 108.8(5) 2_565 2_565 ? 
Mo3 O5 Mo2 102.8(4) . 2_565 ? 
V1 O9 Mo1 112.8(4) . . ? 
V1 O10 Nd1 133.5(5) 2_565 . ? 
V1 O11 V1 103.2(4) 2_565 . ? 
V1 O11 Mo3 90.8(3) 2_565 . ? 
V1 O11 Mo3 98.3(3) . . ? 
V1 O11 Mo2 89.8(3) 2_565 . ? 
V1 O11 Mo2 97.8(4) . . ? 
Mo3 O11 Mo2 163.3(5) . . ? 
V1 O11 Mo1 165.4(5) 2_565 . ? 
V1 O11 Mo1 91.4(3) . . ? 
Mo3 O11 Mo1 87.7(4) . . ? 
Mo2 O11 Mo1 87.6(3) . . ? 
Mo1 O12 Nd1 135.2(5) . . ? 
V1 O13 Mo2 107.7(5) 2_565 . ? 
V1 O13 Mo3 108.6(3) 2_565 2_565 ? 
Mo2 O13 Mo3 103.2(4) . 2_565 ? 
 
_diffrn_measured_fraction_theta_max    0.986 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.986 
_refine_diff_density_max    1.532 
_refine_diff_density_min   -2.093 
_refine_diff_density_rms    0.261 

#=======================END

